# Electronic Supplementary Material (ESI) for New Journal of Chemistry.
# This journal is © The Royal Society of Chemistry and the Centre National de la Recherche Scientifique 2018

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_1
_database_code_depnum_ccdc_archive 'CCDC 1821287'
_audit_update_record             
;
2018-02-01 deposited with the CCDC.
2018-05-10 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
; 
 ? 
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'Li Mo3 O10 Rb'
_chemical_formula_weight         540.23

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Li Li -0.0003 0.0001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Rb Rb -0.9393 2.9676 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           Orthorhombic
_symmetry_space_group_name_H-M   Pnma

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-x, y+1/2, -z'
'x+1/2, -y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, y, -z-1/2'
'x, -y-1/2, z'
'-x-1/2, y-1/2, z-1/2'

_cell_length_a                   8.532(8)
_cell_length_b                   7.552(7)
_cell_length_c                   13.582(12)
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_volume                     875.1(13)
_cell_formula_units_Z            4
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    1185
_cell_measurement_theta_min      2.82
_cell_measurement_theta_max      27.63

_exptl_crystal_description       block
_exptl_crystal_colour            colourless
_exptl_crystal_size_max          0.106
_exptl_crystal_size_mid          0.068
_exptl_crystal_size_min          0.063
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    4.100
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             984
_exptl_absorpt_coefficient_mu    9.794
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_correction_T_min  0.8039
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_process_details   ?

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            5154
_diffrn_reflns_av_R_equivalents  0.0438
_diffrn_reflns_av_sigmaI/netI    0.0345
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_theta_min         2.82
_diffrn_reflns_theta_max         27.82
_reflns_number_total             1103
_reflns_number_gt                875
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0117P)²+0.5710P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   ?
_refine_ls_hydrogen_treatment    ?
_refine_ls_extinction_method     SHELXL
_refine_ls_extinction_coef       0.00240(11)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_number_reflns         1103
_refine_ls_number_parameters     80
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0364
_refine_ls_R_factor_gt           0.0243
_refine_ls_wR_factor_ref         0.0451
_refine_ls_wR_factor_gt          0.0418
_refine_ls_goodness_of_fit_ref   1.051
_refine_ls_restrained_S_all      1.051
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.17737(6) 0.2500 0.40474(4) 0.00928(13) Uani 1 2 d S . .
Mo2 Mo -0.13065(4) -0.00108(4) 0.39722(2) 0.00911(10) Uani 1 1 d . . .
Rb1 Rb 0.39468(8) -0.2500 0.40239(5) 0.02619(18) Uani 1 2 d S . .
Li1 Li 0.0514(17) 0.2500 0.1599(8) 0.036(3) Uani 1 2 d S . .
O1 O 0.1178(3) 0.0119(3) 0.43666(18) 0.0094(6) Uani 1 1 d . . .
O2 O -0.0807(5) 0.2500 0.4114(3) 0.0100(8) Uani 1 2 d S . .
O3 O -0.1299(5) -0.2500 0.4325(3) 0.0103(9) Uani 1 2 d S . .
O4 O 0.3759(5) 0.2500 0.4282(3) 0.0161(10) Uani 1 2 d S . .
O5 O 0.1627(5) 0.2500 0.2800(3) 0.0161(9) Uani 1 2 d S . .
O6 O -0.3275(3) 0.0401(4) 0.4040(2) 0.0167(6) Uani 1 1 d . . .
O7 O -0.0932(3) -0.0299(4) 0.2760(2) 0.0187(7) Uani 1 1 d . . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O5 1.699(4) . ?
Mo1 O4 1.724(4) . ?
Mo1 O1 1.918(3) 7_565 ?
Mo1 O1 1.918(3) . ?
Mo1 O2 2.203(4) . ?
Mo1 O3 2.247(4) 5_556 ?
Mo1 Li1 3.309(14) 6_656 ?
Mo1 Rb1 4.207(3) 1_565 ?
Mo1 Rb1 4.207(3) . ?
Mo2 O7 1.691(3) . ?
Mo2 O6 1.711(3) . ?
Mo2 O3 1.9400(19) . ?
Mo2 O2 1.9529(19) . ?
Mo2 O1 2.189(3) . ?
Mo2 O1 2.260(3) 5_556 ?
Mo2 Rb1 4.010(2) 5_556 ?
Rb1 O7 2.940(3) 4_545 ?
Rb1 O7 2.940(3) 6_656 ?
Rb1 O4 3.021(5) 5_656 ?
Rb1 O1 3.116(3) 7 ?
Rb1 O1 3.116(3) . ?
Rb1 O6 3.123(4) 5_556 ?
Rb1 O6 3.123(4) 3_546 ?
Rb1 O6 3.228(4) 1_655 ?
Rb1 O6 3.228(4) 7_655 ?
Rb1 Li1 3.527(12) 2 ?
Rb1 Mo2 4.010(2) 5_556 ?
Rb1 Mo2 4.010(2) 3_546 ?
Li1 O5 1.888(13) . ?
Li1 O4 1.916(14) 6_556 ?
Li1 O6 2.082(9) 4 ?
Li1 O6 2.082(9) 6_656 ?
Li1 Mo1 3.309(14) 6_556 ?
Li1 Rb1 3.527(12) 2_554 ?
Li1 Rb1 4.094(6) 6_556 ?
Li1 Rb1 4.094(6) 6_566 ?
O1 Mo2 2.260(3) 5_556 ?
O2 Mo2 1.9529(19) 7_565 ?
O3 Mo2 1.9400(19) 7 ?
O3 Mo1 2.247(4) 5_556 ?
O4 Li1 1.916(14) 6_656 ?
O4 Rb1 3.021(5) 5_656 ?
O6 Li1 2.082(9) 6_556 ?
O6 Rb1 3.123(4) 5_556 ?
O6 Rb1 3.228(4) 1_455 ?
O7 Rb1 2.940(3) 6_556 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O5 Mo1 O4 104.9(2) . . ?
O5 Mo1 O1 101.88(9) . 7_565 ?
O4 Mo1 O1 102.63(9) . 7_565 ?
O5 Mo1 O1 101.88(9) . . ?
O4 Mo1 O1 102.63(9) . . ?
O1 Mo1 O1 139.24(17) 7_565 . ?
O5 Mo1 O2 88.11(17) . . ?
O4 Mo1 O2 167.00(17) . . ?
O1 Mo1 O2 74.10(9) 7_565 . ?
O1 Mo1 O2 74.10(9) . . ?
O5 Mo1 O3 165.37(18) . 5_556 ?
O4 Mo1 O3 89.75(17) . 5_556 ?
O1 Mo1 O3 74.33(8) 7_565 5_556 ?
O1 Mo1 O3 74.33(8) . 5_556 ?
O2 Mo1 O3 77.26(14) . 5_556 ?
O5 Mo1 Li1 78.9(3) . 6_656 ?
O4 Mo1 Li1 26.0(2) . 6_656 ?
O1 Mo1 Li1 108.38(9) 7_565 6_656 ?
O1 Mo1 Li1 108.38(9) . 6_656 ?
O2 Mo1 Li1 167.0(2) . 6_656 ?
O3 Mo1 Li1 115.8(2) 5_556 6_656 ?
O5 Mo1 Rb1 91.43(6) . 1_565 ?
O4 Mo1 Rb1 64.42(3) . 1_565 ?
O1 Mo1 Rb1 43.71(9) 7_565 1_565 ?
O1 Mo1 Rb1 163.72(8) . 1_565 ?
O2 Mo1 Rb1 116.15(3) . 1_565 ?
O3 Mo1 Rb1 94.99(5) 5_556 1_565 ?
Li1 Mo1 Rb1 64.72(4) 6_656 1_565 ?
O5 Mo1 Rb1 91.43(6) . . ?
O4 Mo1 Rb1 64.42(3) . . ?
O1 Mo1 Rb1 163.72(8) 7_565 . ?
O1 Mo1 Rb1 43.71(9) . . ?
O2 Mo1 Rb1 116.15(3) . . ?
O3 Mo1 Rb1 94.99(5) 5_556 . ?
Li1 Mo1 Rb1 64.72(4) 6_656 . ?
Rb1 Mo1 Rb1 127.68(6) 1_565 . ?
O7 Mo2 O6 105.17(14) . . ?
O7 Mo2 O3 96.61(15) . . ?
O6 Mo2 O3 99.56(15) . . ?
O7 Mo2 O2 100.35(14) . . ?
O6 Mo2 O2 91.88(15) . . ?
O3 Mo2 O2 156.29(16) . . ?
O7 Mo2 O1 93.49(13) . . ?
O6 Mo2 O1 158.38(12) . . ?
O3 Mo2 O1 88.83(13) . . ?
O2 Mo2 O1 73.79(13) . . ?
O7 Mo2 O1 163.31(12) . 5_556 ?
O6 Mo2 O1 90.01(12) . 5_556 ?
O3 Mo2 O1 73.62(13) . 5_556 ?
O2 Mo2 O1 85.77(12) . 5_556 ?
O1 Mo2 O1 73.16(11) . 5_556 ?
O7 Mo2 Rb1 145.88(10) . 5_556 ?
O6 Mo2 Rb1 47.60(10) . 5_556 ?
O3 Mo2 Rb1 107.00(12) . 5_556 ?
O2 Mo2 Rb1 66.22(12) . 5_556 ?
O1 Mo2 Rb1 110.91(8) . 5_556 ?
O1 Mo2 Rb1 50.71(8) 5_556 5_556 ?
O7 Rb1 O7 68.85(13) 4_545 6_656 ?
O7 Rb1 O4 127.22(9) 4_545 5_656 ?
O7 Rb1 O4 127.22(9) 6_656 5_656 ?
O7 Rb1 O1 77.93(8) 4_545 7 ?
O7 Rb1 O1 120.57(8) 6_656 7 ?
O4 Rb1 O1 112.17(9) 5_656 7 ?
O7 Rb1 O1 120.57(8) 4_545 . ?
O7 Rb1 O1 77.93(8) 6_656 . ?
O4 Rb1 O1 112.17(9) 5_656 . ?
O1 Rb1 O1 78.80(12) 7 . ?
O7 Rb1 O6 170.82(8) 4_545 5_556 ?
O7 Rb1 O6 114.41(10) 6_656 5_556 ?
O4 Rb1 O6 58.51(10) 5_656 5_556 ?
O1 Rb1 O6 93.29(8) 7 5_556 ?
O1 Rb1 O6 54.05(7) . 5_556 ?
O7 Rb1 O6 114.41(10) 4_545 3_546 ?
O7 Rb1 O6 170.82(8) 6_656 3_546 ?
O4 Rb1 O6 58.51(10) 5_656 3_546 ?
O1 Rb1 O6 54.05(7) 7 3_546 ?
O1 Rb1 O6 93.28(8) . 3_546 ?
O6 Rb1 O6 61.01(12) 5_556 3_546 ?
O7 Rb1 O6 111.32(8) 4_545 1_655 ?
O7 Rb1 O6 66.18(8) 6_656 1_655 ?
O4 Rb1 O6 61.24(8) 5_656 1_655 ?
O1 Rb1 O6 170.59(7) 7 1_655 ?
O1 Rb1 O6 97.18(10) . 1_655 ?
O6 Rb1 O6 77.55(9) 5_556 1_655 ?
O6 Rb1 O6 118.26(5) 3_546 1_655 ?
O7 Rb1 O6 66.18(8) 4_545 7_655 ?
O7 Rb1 O6 111.32(8) 6_656 7_655 ?
O4 Rb1 O6 61.24(8) 5_656 7_655 ?
O1 Rb1 O6 97.18(10) 7 7_655 ?
O1 Rb1 O6 170.59(7) . 7_655 ?
O6 Rb1 O6 118.26(5) 5_556 7_655 ?
O6 Rb1 O6 77.55(9) 3_546 7_655 ?
O6 Rb1 O6 85.48(13) 1_655 7_655 ?
O7 Rb1 Li1 144.34(9) 4_545 2 ?
O7 Rb1 Li1 144.34(9) 6_656 2 ?
O4 Rb1 Li1 32.9(2) 5_656 2 ?
O1 Rb1 Li1 87.18(19) 7 2 ?
O1 Rb1 Li1 87.18(19) . 2 ?
O6 Rb1 Li1 35.84(13) 5_556 2 ?
O6 Rb1 Li1 35.84(13) 3_546 2 ?
O6 Rb1 Li1 84.10(18) 1_655 2 ?
O6 Rb1 Li1 84.10(18) 7_655 2 ?
O7 Rb1 Mo2 147.83(7) 4_545 5_556 ?
O7 Rb1 Mo2 108.17(8) 6_656 5_556 ?
O4 Rb1 Mo2 81.20(9) 5_656 5_556 ?
O1 Rb1 Mo2 76.87(7) 7 5_556 ?
O1 Rb1 Mo2 34.16(5) . 5_556 ?
O6 Rb1 Mo2 23.86(6) 5_556 5_556 ?
O6 Rb1 Mo2 64.25(8) 3_546 5_556 ?
O6 Rb1 Mo2 94.99(7) 1_655 5_556 ?
O6 Rb1 Mo2 136.79(6) 7_655 5_556 ?
Li1 Rb1 Mo2 53.16(19) 2 5_556 ?
O7 Rb1 Mo2 108.17(8) 4_545 3_546 ?
O7 Rb1 Mo2 147.83(7) 6_656 3_546 ?
O4 Rb1 Mo2 81.20(9) 5_656 3_546 ?
O1 Rb1 Mo2 34.16(5) 7 3_546 ?
O1 Rb1 Mo2 76.87(7) . 3_546 ?
O6 Rb1 Mo2 64.25(8) 5_556 3_546 ?
O6 Rb1 Mo2 23.86(6) 3_546 3_546 ?
O6 Rb1 Mo2 136.79(6) 1_655 3_546 ?
O6 Rb1 Mo2 94.99(7) 7_655 3_546 ?
Li1 Rb1 Mo2 53.16(19) 2 3_546 ?
Mo2 Rb1 Mo2 56.44(5) 5_556 3_546 ?
O5 Li1 O4 158.8(8) . 6_556 ?
O5 Li1 O6 96.4(5) . 4 ?
O4 Li1 O6 97.3(4) 6_556 4 ?
O5 Li1 O6 96.4(5) . 6_656 ?
O4 Li1 O6 97.3(4) 6_556 6_656 ?
O6 Li1 O6 99.2(6) 4 6_656 ?
O5 Li1 Mo1 135.6(6) . 6_556 ?
O4 Li1 Mo1 23.2(2) 6_556 6_556 ?
O6 Li1 Mo1 111.6(4) 4 6_556 ?
O6 Li1 Mo1 111.6(4) 6_656 6_556 ?
O5 Li1 Rb1 142.3(6) . 2_554 ?
O4 Li1 Rb1 58.9(3) 6_556 2_554 ?
O6 Li1 Rb1 61.4(3) 4 2_554 ?
O6 Li1 Rb1 61.4(3) 6_656 2_554 ?
Mo1 Li1 Rb1 82.1(3) 6_556 2_554 ?
O5 Li1 Rb1 110.05(17) . 6_556 ?
O4 Li1 Rb1 67.42(18) 6_556 6_556 ?
O6 Li1 Rb1 141.1(4) 4 6_556 ?
O6 Li1 Rb1 51.22(18) 6_656 6_556 ?
Mo1 Li1 Rb1 68.31(18) 6_556 6_556 ?
Rb1 Li1 Rb1 80.67(17) 2_554 6_556 ?
O5 Li1 Rb1 110.05(17) . 6_566 ?
O4 Li1 Rb1 67.42(18) 6_556 6_566 ?
O6 Li1 Rb1 51.22(18) 4 6_566 ?
O6 Li1 Rb1 141.1(4) 6_656 6_566 ?
Mo1 Li1 Rb1 68.31(18) 6_556 6_566 ?
Rb1 Li1 Rb1 80.67(17) 2_554 6_566 ?
Rb1 Li1 Rb1 134.5(4) 6_556 6_566 ?
Mo1 O1 Mo2 104.08(12) . . ?
Mo1 O1 Mo2 104.28(11) . 5_556 ?
Mo2 O1 Mo2 106.84(11) . 5_556 ?
Mo1 O1 Rb1 111.12(12) . . ?
Mo2 O1 Rb1 132.02(11) . . ?
Mo2 O1 Rb1 95.13(9) 5_556 . ?
Mo2 O2 Mo2 152.3(2) . 7_565 ?
Mo2 O2 Mo1 102.37(12) . . ?
Mo2 O2 Mo1 102.37(12) 7_565 . ?
Mo2 O3 Mo2 151.4(2) 7 . ?
Mo2 O3 Mo1 104.03(11) 7 5_556 ?
Mo2 O3 Mo1 104.03(11) . 5_556 ?
Mo1 O4 Li1 130.7(4) . 6_656 ?
Mo1 O4 Rb1 141.0(2) . 5_656 ?
Li1 O4 Rb1 88.2(4) 6_656 5_656 ?
Mo1 O5 Li1 154.0(5) . . ?
Mo2 O6 Li1 127.1(4) . 6_556 ?
Mo2 O6 Rb1 108.54(12) . 5_556 ?
Li1 O6 Rb1 82.7(3) 6_556 5_556 ?
Mo2 O6 Rb1 126.69(14) . 1_455 ?
Li1 O6 Rb1 98.6(3) 6_556 1_455 ?
Rb1 O6 Rb1 102.45(9) 5_556 1_455 ?
Mo2 O7 Rb1 150.28(15) . 6_556 ?

_diffrn_measured_fraction_theta_max 0.991
_diffrn_reflns_theta_full        27.82
_diffrn_measured_fraction_theta_full 0.991
_refine_diff_density_max         0.782
_refine_diff_density_min         -0.749
_refine_diff_density_rms         0.179
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_1_CCDC1
_database_code_depnum_ccdc_archive 'CCDC 1823501'
_audit_update_record             
;
2018-02-11 deposited with the CCDC.
2018-05-10 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
; 
 ? 
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'Cs K Mo3 O10'
_chemical_formula_weight         619.83

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           Triclinic
_symmetry_space_group_name_H-M   P-1

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   8.195(11)
_cell_length_b                   8.224(11)
_cell_length_c                   8.360(12)
_cell_angle_alpha                63.930(13)
_cell_angle_beta                 85.769(16)
_cell_angle_gamma                74.330(15)
_cell_volume                     486.6(12)
_cell_formula_units_Z            2
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    1010
_cell_measurement_theta_min      2.72
_cell_measurement_theta_max      27.16

_exptl_crystal_description       block
_exptl_crystal_colour            colorless
_exptl_crystal_size_max          ?
_exptl_crystal_size_mid          ?
_exptl_crystal_size_min          ?
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    4.230
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             560
_exptl_absorpt_coefficient_mu    7.955
_exptl_absorpt_correction_type   none
_exptl_absorpt_correction_T_min  0.6032
_exptl_absorpt_correction_T_max  0.7456
_exptl_absorpt_process_details   ?

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            2975
_diffrn_reflns_av_R_equivalents  0.0227
_diffrn_reflns_av_sigmaI/netI    0.0525
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_theta_min         2.72
_diffrn_reflns_theta_max         27.43
_reflns_number_total             2134
_reflns_number_gt                1734
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0315P)²+9.1794P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   ?
_refine_ls_hydrogen_treatment    ?
_refine_ls_extinction_method     SHELXL
_refine_ls_extinction_coef       0.0055(6)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_number_reflns         2134
_refine_ls_number_parameters     137
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0515
_refine_ls_R_factor_gt           0.0393
_refine_ls_wR_factor_ref         0.1069
_refine_ls_wR_factor_gt          0.0965
_refine_ls_goodness_of_fit_ref   1.127
_refine_ls_restrained_S_all      1.127
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
K1 K -0.8456(3) 0.4782(3) -0.2758(3) 0.0219(5) Uani 1 1 d . . .
Cs1 Cs -0.30998(10) 0.26951(11) -0.08641(10) 0.0259(2) Uani 1 1 d . . .
Mo1 Mo -0.03368(11) -0.06846(12) 0.35550(11) 0.0118(2) Uani 1 1 d . . .
Mo2 Mo 0.44965(11) -0.19855(12) 0.53547(12) 0.0130(2) Uani 1 1 d . . .
Mo3 Mo 0.22782(11) 0.16483(12) 0.19024(11) 0.0125(2) Uani 1 1 d . . .
O1 O 0.4049(9) 0.1000(9) 0.3681(9) 0.0118(14) Uani 1 1 d . . .
O2 O 0.0257(9) 0.1541(9) 0.3993(9) 0.0116(14) Uani 1 1 d . . .
O3 O 0.2627(9) -0.1315(10) 0.3878(10) 0.0150(15) Uani 1 1 d . . .
O4 O 0.0464(10) 0.0959(10) 0.1319(9) 0.0160(15) Uani 1 1 d . . .
O5 O 0.4155(10) -0.3751(10) 0.7303(10) 0.0229(18) Uani 1 1 d . . .
O6 O 0.0112(10) -0.2756(11) 0.3350(10) 0.0211(17) Uani 1 1 d . . .
O7 O 0.1625(10) 0.3989(11) 0.1169(11) 0.0240(18) Uani 1 1 d . . .
O8 O -0.2449(10) 0.0266(11) 0.3093(10) 0.0237(18) Uani 1 1 d . . .
O9 O -0.3537(11) -0.1430(12) -0.0259(11) 0.0253(18) Uani 1 1 d . . .
O10 O 0.6007(10) -0.3080(12) 0.4397(13) 0.030(2) Uani 1 1 d . . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
K1 O6 2.629(8) 2_455 ?
K1 O2 2.731(8) 2_465 ?
K1 O5 2.739(9) 1_464 ?
K1 O10 2.762(9) 2 ?
K1 O9 2.948(9) 2_455 ?
K1 O7 2.964(9) 2_465 ?
K1 O7 3.056(10) 1_455 ?
K1 O6 3.090(9) 1_464 ?
K1 Mo3 3.587(5) 1_455 ?
K1 Mo1 3.643(4) 1_464 ?
K1 Mo2 3.825(4) 1_464 ?
K1 Mo3 3.935(4) 2_465 ?
Cs1 O5 2.995(8) 1_464 ?
Cs1 O8 3.016(9) . ?
Cs1 O6 3.089(8) 2 ?
Cs1 O9 3.142(9) 2_455 ?
Cs1 O3 3.150(8) 2 ?
Cs1 O7 3.176(9) 2_565 ?
Cs1 O4 3.184(8) . ?
Cs1 O9 3.319(10) . ?
Cs1 O4 3.349(8) 2 ?
Cs1 O5 3.443(9) 2_556 ?
Cs1 O10 3.783(10) 2 ?
Cs1 Mo3 3.912(5) 2 ?
Mo1 O8 1.691(9) . ?
Mo1 O6 1.725(8) . ?
Mo1 O2 1.852(7) 2_556 ?
Mo1 O4 1.957(7) . ?
Mo1 O2 2.195(7) . ?
Mo1 O3 2.353(8) . ?
Mo1 Mo3 3.104(3) . ?
Mo1 Mo1 3.215(4) 2_556 ?
Mo1 K1 3.643(4) 1_646 ?
Mo1 Cs1 3.943(4) 2 ?
Mo1 K1 4.080(5) 2_455 ?
Mo2 O10 1.694(8) . ?
Mo2 O5 1.706(7) . ?
Mo2 O3 1.843(8) . ?
Mo2 O1 1.992(7) 2_656 ?
Mo2 O1 2.166(7) . ?
Mo2 K1 3.825(4) 1_646 ?
Mo2 Cs1 4.138(4) 1_646 ?
Mo2 Cs1 4.320(5) 2 ?
Mo2 Cs1 4.482(6) 2_556 ?
Mo3 O7 1.680(8) . ?
Mo3 O9 1.700(8) 2 ?
Mo3 O4 1.891(8) . ?
Mo3 O1 1.950(7) . ?
Mo3 O3 2.214(8) . ?
Mo3 O2 2.307(7) . ?
Mo3 K1 3.587(5) 1_655 ?
Mo3 Cs1 3.912(5) 2 ?
Mo3 K1 3.935(4) 2_465 ?
Mo3 Cs1 4.377(5) 1_655 ?
O1 Mo2 1.992(7) 2_656 ?
O2 Mo1 1.852(7) 2_556 ?
O2 K1 2.731(8) 2_465 ?
O3 Cs1 3.150(8) 2 ?
O4 Cs1 3.349(8) 2 ?
O5 K1 2.739(9) 1_646 ?
O5 Cs1 2.995(8) 1_646 ?
O5 Cs1 3.443(9) 2_556 ?
O6 K1 2.629(8) 2_455 ?
O6 Cs1 3.089(8) 2 ?
O6 K1 3.090(9) 1_646 ?
O7 K1 2.964(9) 2_465 ?
O7 K1 3.056(10) 1_655 ?
O7 Cs1 3.176(9) 2_565 ?
O9 Mo3 1.700(8) 2 ?
O9 K1 2.948(9) 2_455 ?
O9 Cs1 3.142(9) 2_455 ?
O10 K1 2.762(9) 2 ?
O10 Cs1 3.783(10) 2 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O6 K1 O2 112.2(3) 2_455 2_465 ?
O6 K1 O5 159.1(3) 2_455 1_464 ?
O2 K1 O5 81.9(2) 2_465 1_464 ?
O6 K1 O10 79.9(3) 2_455 2 ?
O2 K1 O10 129.3(3) 2_465 2 ?
O5 K1 O10 79.2(3) 1_464 2 ?
O6 K1 O9 91.1(3) 2_455 2_455 ?
O2 K1 O9 146.5(2) 2_465 2_455 ?
O5 K1 O9 83.5(3) 1_464 2_455 ?
O10 K1 O9 76.6(3) 2 2_455 ?
O6 K1 O7 84.5(3) 2_455 2_465 ?
O2 K1 O7 57.5(2) 2_465 2_465 ?
O5 K1 O7 116.4(3) 1_464 2_465 ?
O10 K1 O7 164.4(3) 2 2_465 ?
O9 K1 O7 104.0(2) 2_455 2_465 ?
O6 K1 O7 112.0(2) 2_455 1_455 ?
O2 K1 O7 95.8(2) 2_465 1_455 ?
O5 K1 O7 80.3(2) 1_464 1_455 ?
O10 K1 O7 126.1(3) 2 1_455 ?
O9 K1 O7 51.9(2) 2_455 1_455 ?
O7 K1 O7 60.5(3) 2_465 1_455 ?
O6 K1 O6 76.3(3) 2_455 1_464 ?
O2 K1 O6 56.6(2) 2_465 1_464 ?
O5 K1 O6 101.2(2) 1_464 1_464 ?
O10 K1 O6 81.7(3) 2 1_464 ?
O9 K1 O6 156.6(2) 2_455 1_464 ?
O7 K1 O6 94.5(2) 2_465 1_464 ?
O7 K1 O6 151.3(2) 1_455 1_464 ?
O6 K1 Mo3 92.9(2) 2_455 1_455 ?
O2 K1 Mo3 122.81(16) 2_465 1_455 ?
O5 K1 Mo3 91.70(18) 1_464 1_455 ?
O10 K1 Mo3 104.5(2) 2 1_455 ?
O9 K1 Mo3 28.03(16) 2_455 1_455 ?
O7 K1 Mo3 76.30(17) 2_465 1_455 ?
O7 K1 Mo3 27.85(16) 1_455 1_455 ?
O6 K1 Mo3 166.61(17) 1_464 1_455 ?
O6 K1 Mo1 98.8(2) 2_455 1_464 ?
O2 K1 Mo1 29.60(15) 2_465 1_464 ?
O5 K1 Mo1 86.26(19) 1_464 1_464 ?
O10 K1 Mo1 102.3(2) 2 1_464 ?
O9 K1 Mo1 169.71(19) 2_455 1_464 ?
O7 K1 Mo1 79.93(17) 2_465 1_464 ?
O7 K1 Mo1 125.37(18) 1_455 1_464 ?
O6 K1 Mo1 28.18(14) 1_464 1_464 ?
Mo3 K1 Mo1 152.31(8) 1_455 1_464 ?
O6 K1 Mo2 146.1(2) 2_455 1_464 ?
O2 K1 Mo2 69.28(18) 2_465 1_464 ?
O5 K1 Mo2 23.45(16) 1_464 1_464 ?
O10 K1 Mo2 75.1(2) 2 1_464 ?
O9 K1 Mo2 104.7(2) 2_455 1_464 ?
O7 K1 Mo2 119.06(19) 2_465 1_464 ?
O7 K1 Mo2 101.18(17) 1_455 1_464 ?
O6 K1 Mo2 77.76(16) 1_464 1_464 ?
Mo3 K1 Mo2 115.14(9) 1_455 1_464 ?
Mo1 K1 Mo2 65.33(9) 1_464 1_464 ?
O6 K1 Mo3 99.9(2) 2_455 2_465 ?
O2 K1 Mo3 34.92(14) 2_465 2_465 ?
O5 K1 Mo3 100.2(2) 1_464 2_465 ?
O10 K1 Mo3 162.9(2) 2 2_465 ?
O9 K1 Mo3 120.47(19) 2_455 2_465 ?
O7 K1 Mo3 23.14(15) 2_465 2_465 ?
O7 K1 Mo3 70.04(16) 1_455 2_465 ?
O6 K1 Mo3 81.60(18) 1_464 2_465 ?
Mo3 K1 Mo3 92.67(9) 1_455 2_465 ?
Mo1 K1 Mo3 60.70(9) 1_464 2_465 ?
Mo2 K1 Mo3 97.41(12) 1_464 2_465 ?
O5 Cs1 O8 127.4(2) 1_464 . ?
O5 Cs1 O6 108.3(2) 1_464 2 ?
O8 Cs1 O6 119.4(2) . 2 ?
O5 Cs1 O9 76.2(2) 1_464 2_455 ?
O8 Cs1 O9 77.3(2) . 2_455 ?
O6 Cs1 O9 144.6(2) 2 2_455 ?
O5 Cs1 O3 98.7(2) 1_464 2 ?
O8 Cs1 O3 126.7(2) . 2 ?
O6 Cs1 O3 53.0(2) 2 2 ?
O9 Cs1 O3 91.7(2) 2_455 2 ?
O5 Cs1 O7 73.6(2) 1_464 2_565 ?
O8 Cs1 O7 98.6(2) . 2_565 ?
O6 Cs1 O7 73.9(2) 2 2_565 ?
O9 Cs1 O7 137.9(2) 2_455 2_565 ?
O3 Cs1 O7 121.3(2) 2 2_565 ?
O5 Cs1 O4 143.8(2) 1_464 . ?
O8 Cs1 O4 53.1(2) . . ?
O6 Cs1 O4 68.5(2) 2 . ?
O9 Cs1 O4 128.3(2) 2_455 . ?
O3 Cs1 O4 105.7(2) 2 . ?
O7 Cs1 O4 70.9(2) 2_565 . ?
O5 Cs1 O9 121.7(2) 1_464 . ?
O8 Cs1 O9 75.4(2) . . ?
O6 Cs1 O9 96.1(2) 2 . ?
O9 Cs1 O9 55.8(3) 2_455 . ?
O3 Cs1 O9 56.44(19) 2 . ?
O7 Cs1 O9 164.3(2) 2_565 . ?
O4 Cs1 O9 94.3(2) . . ?
O5 Cs1 O4 144.6(2) 1_464 2 ?
O8 Cs1 O4 85.6(2) . 2 ?
O6 Cs1 O4 52.43(19) 2 2 ?
O9 Cs1 O4 103.2(2) 2_455 2 ?
O3 Cs1 O4 45.96(19) 2 2 ?
O7 Cs1 O4 118.5(2) 2_565 2 ?
O4 Cs1 O4 63.6(2) . 2 ?
O9 Cs1 O4 47.4(2) . 2 ?
O5 Cs1 O5 81.3(2) 1_464 2_556 ?
O8 Cs1 O5 49.1(2) . 2_556 ?
O6 Cs1 O5 136.8(2) 2 2_556 ?
O9 Cs1 O5 78.2(2) 2_455 2_556 ?
O3 Cs1 O5 169.65(18) 2 2_556 ?
O7 Cs1 O5 68.8(2) 2_565 2_556 ?
O4 Cs1 O5 79.3(2) . 2_556 ?
O9 Cs1 O5 114.72(19) . 2_556 ?
O4 Cs1 O5 133.79(18) 2 2_556 ?
O5 Cs1 O10 61.0(2) 1_464 2 ?
O8 Cs1 O10 134.4(2) . 2 ?
O6 Cs1 O10 90.1(2) 2 2 ?
O9 Cs1 O10 60.7(2) 2_455 2 ?
O3 Cs1 O10 45.13(19) 2 2 ?
O7 Cs1 O10 123.9(2) 2_565 2 ?
O4 Cs1 O10 150.47(18) . 2 ?
O9 Cs1 O10 67.0(2) . 2 ?
O4 Cs1 O10 87.35(19) 2 2 ?
O5 Cs1 O10 128.7(2) 2_556 2 ?
O5 Cs1 Mo3 124.07(18) 1_464 2 ?
O8 Cs1 Mo3 92.71(18) . 2 ?
O6 Cs1 Mo3 71.15(15) 2 2 ?
O9 Cs1 Mo3 77.50(16) 2_455 2 ?
O3 Cs1 Mo3 34.45(13) 2 2 ?
O7 Cs1 Mo3 144.43(16) 2_565 2 ?
O4 Cs1 Mo3 90.05(14) . 2 ?
O9 Cs1 Mo3 25.54(14) . 2 ?
O4 Cs1 Mo3 28.88(14) 2 2 ?
O5 Cs1 Mo3 138.43(12) 2_556 2 ?
O10 Cs1 Mo3 63.05(13) 2 2 ?
O8 Mo1 O6 105.7(4) . . ?
O8 Mo1 O2 100.1(3) . 2_556 ?
O6 Mo1 O2 101.8(3) . 2_556 ?
O8 Mo1 O4 98.7(4) . . ?
O6 Mo1 O4 101.4(3) . . ?
O2 Mo1 O4 144.7(3) 2_556 . ?
O8 Mo1 O2 98.5(3) . . ?
O6 Mo1 O2 155.7(3) . . ?
O2 Mo1 O2 75.1(3) 2_556 . ?
O4 Mo1 O2 72.7(3) . . ?
O8 Mo1 O3 167.4(3) . . ?
O6 Mo1 O3 84.7(3) . . ?
O2 Mo1 O3 84.4(3) 2_556 . ?
O4 Mo1 O3 71.7(3) . . ?
O2 Mo1 O3 71.1(3) . . ?
O8 Mo1 Mo3 122.3(3) . . ?
O6 Mo1 Mo3 114.4(3) . . ?
O2 Mo1 Mo3 109.8(2) 2_556 . ?
O4 Mo1 Mo3 35.5(2) . . ?
O2 Mo1 Mo3 47.92(18) . . ?
O3 Mo1 Mo3 45.33(18) . . ?
O8 Mo1 Mo1 101.7(3) . 2_556 ?
O6 Mo1 Mo1 137.8(3) . 2_556 ?
O2 Mo1 Mo1 41.3(2) 2_556 2_556 ?
O4 Mo1 Mo1 105.5(2) . 2_556 ?
O2 Mo1 Mo1 33.83(17) . 2_556 ?
O3 Mo1 Mo1 73.88(18) . 2_556 ?
Mo3 Mo1 Mo1 74.76(8) . 2_556 ?
O8 Mo1 K1 124.1(3) . 1_646 ?
O6 Mo1 K1 57.8(3) . 1_646 ?
O2 Mo1 K1 46.8(2) 2_556 1_646 ?
O4 Mo1 K1 135.2(2) . 1_646 ?
O2 Mo1 K1 109.3(2) . 1_646 ?
O3 Mo1 K1 67.46(18) . 1_646 ?
Mo3 Mo1 K1 112.21(10) . 1_646 ?
Mo1 Mo1 K1 80.27(12) 2_556 1_646 ?
O8 Mo1 Cs1 46.7(3) . . ?
O6 Mo1 Cs1 99.7(3) . . ?
O2 Mo1 Cs1 144.7(2) 2_556 . ?
O4 Mo1 Cs1 54.0(2) . . ?
O2 Mo1 Cs1 95.6(2) . . ?
O3 Mo1 Cs1 125.41(18) . . ?
Mo3 Mo1 Cs1 85.92(9) . . ?
Mo1 Mo1 Cs1 122.46(10) 2_556 . ?
K1 Mo1 Cs1 155.00(5) 1_646 . ?
O8 Mo1 Cs1 129.2(3) . 2 ?
O6 Mo1 Cs1 48.7(3) . 2 ?
O2 Mo1 Cs1 125.2(2) 2_556 2 ?
O4 Mo1 Cs1 58.1(2) . 2 ?
O2 Mo1 Cs1 113.02(19) . 2 ?
O3 Mo1 Cs1 53.02(18) . 2 ?
Mo3 Mo1 Cs1 66.21(9) . 2 ?
Mo1 Mo1 Cs1 126.79(8) 2_556 2 ?
K1 Mo1 Cs1 82.49(11) 1_646 2 ?
Cs1 Mo1 Cs1 89.97(11) . 2 ?
O8 Mo1 K1 80.4(3) . 2_455 ?
O6 Mo1 K1 25.4(3) . 2_455 ?
O2 Mo1 K1 104.6(2) 2_556 2_455 ?
O4 Mo1 K1 107.8(2) . 2_455 ?
O2 Mo1 K1 178.81(19) . 2_455 ?
O3 Mo1 K1 110.08(18) . 2_455 ?
Mo3 Mo1 K1 133.06(7) . 2_455 ?
Mo1 Mo1 K1 145.92(6) 2_556 2_455 ?
K1 Mo1 K1 71.14(12) 1_646 2_455 ?
Cs1 Mo1 K1 83.92(10) . 2_455 ?
Cs1 Mo1 K1 68.09(8) 2 2_455 ?
O10 Mo2 O5 104.6(4) . . ?
O10 Mo2 O3 100.6(4) . . ?
O5 Mo2 O3 104.7(4) . . ?
O10 Mo2 O1 98.9(4) . 2_656 ?
O5 Mo2 O1 99.0(4) . 2_656 ?
O3 Mo2 O1 144.1(3) . 2_656 ?
O10 Mo2 O1 106.6(4) . . ?
O5 Mo2 O1 148.4(3) . . ?
O3 Mo2 O1 74.1(3) . . ?
O1 Mo2 O1 71.6(3) 2_656 . ?
O10 Mo2 K1 104.0(3) . 1_646 ?
O5 Mo2 K1 39.7(3) . 1_646 ?
O3 Mo2 K1 65.7(2) . 1_646 ?
O1 Mo2 K1 136.6(2) 2_656 1_646 ?
O1 Mo2 K1 132.9(2) . 1_646 ?
O10 Mo2 Cs1 70.3(3) . 1_646 ?
O5 Mo2 Cs1 38.4(3) . 1_646 ?
O3 Mo2 Cs1 127.3(2) . 1_646 ?
O1 Mo2 Cs1 87.6(2) 2_656 1_646 ?
O1 Mo2 Cs1 158.46(19) . 1_646 ?
K1 Mo2 Cs1 66.81(10) 1_646 1_646 ?
O10 Mo2 Cs1 60.4(3) . 2 ?
O5 Mo2 Cs1 110.1(3) . 2 ?
O3 Mo2 Cs1 40.3(2) . 2 ?
O1 Mo2 Cs1 147.4(2) 2_656 2 ?
O1 Mo2 Cs1 89.6(2) . 2 ?
K1 Mo2 Cs1 75.57(8) 1_646 2 ?
Cs1 Mo2 Cs1 106.02(10) 1_646 2 ?
O10 Mo2 Cs1 137.8(3) . 2_556 ?
O5 Mo2 Cs1 43.2(3) . 2_556 ?
O3 Mo2 Cs1 112.5(2) . 2_556 ?
O1 Mo2 Cs1 68.9(2) 2_656 2_556 ?
O1 Mo2 Cs1 107.01(19) . 2_556 ?
K1 Mo2 Cs1 69.34(5) 1_646 2_556 ?
Cs1 Mo2 Cs1 69.03(7) 1_646 2_556 ?
Cs1 Mo2 Cs1 143.53(7) 2 2_556 ?
O7 Mo3 O9 102.1(4) . 2 ?
O7 Mo3 O4 105.7(4) . . ?
O9 Mo3 O4 96.3(4) 2 . ?
O7 Mo3 O1 100.7(4) . . ?
O9 Mo3 O1 98.6(4) 2 . ?
O4 Mo3 O1 146.1(3) . . ?
O7 Mo3 O3 155.3(3) . . ?
O9 Mo3 O3 102.1(3) 2 . ?
O4 Mo3 O3 76.1(3) . . ?
O1 Mo3 O3 71.0(3) . . ?
O7 Mo3 O2 85.5(3) . . ?
O9 Mo3 O2 167.0(3) 2 . ?
O4 Mo3 O2 71.3(3) . . ?
O1 Mo3 O2 90.2(3) . . ?
O3 Mo3 O2 71.6(3) . . ?
O7 Mo3 Mo1 118.7(3) . . ?
O9 Mo3 Mo1 122.3(3) 2 . ?
O4 Mo3 Mo1 36.9(2) . . ?
O1 Mo3 Mo1 110.7(2) . . ?
O3 Mo3 Mo1 49.09(19) . . ?
O2 Mo3 Mo1 44.93(17) . . ?
O7 Mo3 K1 58.2(3) . 1_655 ?
O9 Mo3 K1 54.6(3) 2 1_655 ?
O4 Mo3 K1 79.3(2) . 1_655 ?
O1 Mo3 K1 133.6(2) . 1_655 ?
O3 Mo3 K1 143.75(19) . 1_655 ?
O2 Mo3 K1 124.2(2) . 1_655 ?
Mo1 Mo3 K1 115.61(7) . 1_655 ?
O7 Mo3 Cs1 148.5(3) . 2 ?
O9 Mo3 Cs1 57.3(3) 2 2 ?
O4 Mo3 Cs1 58.8(2) . 2 ?
O1 Mo3 Cs1 105.6(2) . 2 ?
O3 Mo3 Cs1 53.6(2) . 2 ?
O2 Mo3 Cs1 111.12(17) . 2 ?
Mo1 Mo3 Cs1 67.24(7) . 2 ?
K1 Mo3 Cs1 90.83(11) 1_655 2 ?
O7 Mo3 K1 43.9(3) . 2_465 ?
O9 Mo3 K1 141.4(3) 2 2_465 ?
O4 Mo3 K1 80.9(3) . 2_465 ?
O1 Mo3 K1 104.8(2) . 2_465 ?
O3 Mo3 K1 114.3(2) . 2_465 ?
O2 Mo3 K1 42.66(18) . 2_465 ?
Mo1 Mo3 K1 77.04(11) . 2_465 ?
K1 Mo3 K1 87.33(9) 1_655 2_465 ?
Cs1 Mo3 K1 139.26(7) 2 2_465 ?
O7 Mo3 Cs1 85.1(3) . 1_655 ?
O9 Mo3 Cs1 35.1(3) 2 1_655 ?
O4 Mo3 Cs1 130.8(2) . 1_655 ?
O1 Mo3 Cs1 71.8(2) . 1_655 ?
O3 Mo3 Cs1 112.74(19) . 1_655 ?
O2 Mo3 Cs1 157.75(18) . 1_655 ?
Mo1 Mo3 Cs1 153.90(5) . 1_655 ?
K1 Mo3 Cs1 66.07(7) 1_655 1_655 ?
Cs1 Mo3 Cs1 86.89(5) 2 1_655 ?
K1 Mo3 Cs1 128.39(8) 2_465 1_655 ?
Mo3 O1 Mo2 145.5(4) . 2_656 ?
Mo3 O1 Mo2 106.0(3) . . ?
Mo2 O1 Mo2 108.4(3) 2_656 . ?
Mo1 O2 Mo1 104.9(3) 2_556 . ?
Mo1 O2 Mo3 134.4(4) 2_556 . ?
Mo1 O2 Mo3 87.2(2) . . ?
Mo1 O2 K1 103.6(3) 2_556 2_465 ?
Mo1 O2 K1 127.9(3) . 2_465 ?
Mo3 O2 K1 102.4(2) . 2_465 ?
Mo2 O3 Mo3 108.0(3) . . ?
Mo2 O3 Mo1 147.8(4) . . ?
Mo3 O3 Mo1 85.6(3) . . ?
Mo2 O3 Cs1 117.4(3) . 2 ?
Mo3 O3 Cs1 92.0(3) . 2 ?
Mo1 O3 Cs1 90.3(2) . 2 ?
Mo3 O4 Mo1 107.5(4) . . ?
Mo3 O4 Cs1 142.1(3) . . ?
Mo1 O4 Cs1 96.2(3) . . ?
Mo3 O4 Cs1 92.3(3) . 2 ?
Mo1 O4 Cs1 92.2(3) . 2 ?
Cs1 O4 Cs1 116.4(2) . 2 ?
Mo2 O5 K1 116.8(4) . 1_646 ?
Mo2 O5 Cs1 120.8(4) . 1_646 ?
K1 O5 Cs1 99.9(3) 1_646 1_646 ?
Mo2 O5 Cs1 116.9(4) . 2_556 ?
K1 O5 Cs1 100.0(2) 1_646 2_556 ?
Cs1 O5 Cs1 98.7(2) 1_646 2_556 ?
Mo1 O6 K1 138.3(4) . 2_455 ?
Mo1 O6 Cs1 106.5(3) . 2 ?
K1 O6 Cs1 103.3(3) 2_455 2 ?
Mo1 O6 K1 94.0(3) . 1_646 ?
K1 O6 K1 103.7(3) 2_455 1_646 ?
Cs1 O6 K1 108.2(3) 2 1_646 ?
Mo3 O7 K1 112.9(4) . 2_465 ?
Mo3 O7 K1 94.0(3) . 1_655 ?
K1 O7 K1 119.5(3) 2_465 1_655 ?
Mo3 O7 Cs1 138.5(4) . 2_565 ?
K1 O7 Cs1 94.0(2) 2_465 2_565 ?
K1 O7 Cs1 99.5(2) 1_655 2_565 ?
Mo1 O8 Cs1 109.2(3) . . ?
Mo3 O9 K1 97.4(4) 2 2_455 ?
Mo3 O9 Cs1 126.8(4) 2 2_455 ?
K1 O9 Cs1 92.2(2) 2_455 2_455 ?
Mo3 O9 Cs1 97.1(3) 2 . ?
K1 O9 Cs1 116.9(3) 2_455 . ?
Cs1 O9 Cs1 124.2(3) 2_455 . ?
Mo2 O10 K1 178.6(5) . 2 ?
Mo2 O10 Cs1 96.7(3) . 2 ?
K1 O10 Cs1 82.7(2) 2 2 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O5 Cs1 Mo1 O8 51.3(5) 1_464 . . . ?
O6 Cs1 Mo1 O8 -174.7(4) 2 . . . ?
O9 Cs1 Mo1 O8 -27.1(4) 2_455 . . . ?
O3 Cs1 Mo1 O8 -123.3(4) 2 . . . ?
O7 Cs1 Mo1 O8 111.5(4) 2_565 . . . ?
O4 Cs1 Mo1 O8 160.3(5) . . . . ?
O9 Cs1 Mo1 O8 -79.5(4) . . . . ?
O4 Cs1 Mo1 O8 -128.0(4) 2 . . . ?
O5 Cs1 Mo1 O8 45.2(4) 2_556 . . . ?
O10 Cs1 Mo1 O8 -76.5(4) 2 . . . ?
Mo3 Cs1 Mo1 O8 -104.0(4) 2 . . . ?
O5 Cs1 Mo1 O6 153.8(4) 1_464 . . . ?
O8 Cs1 Mo1 O6 102.5(5) . . . . ?
O6 Cs1 Mo1 O6 -72.2(3) 2 . . . ?
O9 Cs1 Mo1 O6 75.3(3) 2_455 . . . ?
O3 Cs1 Mo1 O6 -20.8(3) 2 . . . ?
O7 Cs1 Mo1 O6 -146.0(3) 2_565 . . . ?
O4 Cs1 Mo1 O6 -97.2(4) . . . . ?
O9 Cs1 Mo1 O6 23.0(3) . . . . ?
O4 Cs1 Mo1 O6 -25.5(3) 2 . . . ?
O5 Cs1 Mo1 O6 147.7(3) 2_556 . . . ?
O10 Cs1 Mo1 O6 26.0(3) 2 . . . ?
Mo3 Cs1 Mo1 O6 -1.5(3) 2 . . . ?
O5 Cs1 Mo1 O2 27.0(4) 1_464 . . 2_556 ?
O8 Cs1 Mo1 O2 -24.4(5) . . . 2_556 ?
O6 Cs1 Mo1 O2 161.0(4) 2 . . 2_556 ?
O9 Cs1 Mo1 O2 -51.5(4) 2_455 . . 2_556 ?
O3 Cs1 Mo1 O2 -147.7(4) 2 . . 2_556 ?
O7 Cs1 Mo1 O2 87.1(4) 2_565 . . 2_556 ?
O4 Cs1 Mo1 O2 136.0(5) . . . 2_556 ?
O9 Cs1 Mo1 O2 -103.9(4) . . . 2_556 ?
O4 Cs1 Mo1 O2 -152.4(4) 2 . . 2_556 ?
O5 Cs1 Mo1 O2 20.8(4) 2_556 . . 2_556 ?
O10 Cs1 Mo1 O2 -100.8(4) 2 . . 2_556 ?
Mo3 Cs1 Mo1 O2 -128.3(4) 2 . . 2_556 ?
O5 Cs1 Mo1 O4 -109.0(4) 1_464 . . . ?
O8 Cs1 Mo1 O4 -160.3(5) . . . . ?
O6 Cs1 Mo1 O4 25.0(3) 2 . . . ?
O9 Cs1 Mo1 O4 172.5(3) 2_455 . . . ?
O3 Cs1 Mo1 O4 76.3(3) 2 . . . ?
O7 Cs1 Mo1 O4 -48.8(3) 2_565 . . . ?
O9 Cs1 Mo1 O4 120.2(3) . . . . ?
O4 Cs1 Mo1 O4 71.6(3) 2 . . . ?
O5 Cs1 Mo1 O4 -115.1(3) 2_556 . . . ?
O10 Cs1 Mo1 O4 123.2(3) 2 . . . ?
Mo3 Cs1 Mo1 O4 95.7(3) 2 . . . ?
O5 Cs1 Mo1 O2 -45.1(3) 1_464 . . . ?
O8 Cs1 Mo1 O2 -96.4(4) . . . . ?
O6 Cs1 Mo1 O2 88.9(2) 2 . . . ?
O9 Cs1 Mo1 O2 -123.6(2) 2_455 . . . ?
O3 Cs1 Mo1 O2 140.2(2) 2 . . . ?
O7 Cs1 Mo1 O2 15.0(2) 2_565 . . . ?
O4 Cs1 Mo1 O2 63.9(3) . . . . ?
O9 Cs1 Mo1 O2 -176.0(2) . . . . ?
O4 Cs1 Mo1 O2 135.5(2) 2 . . . ?
O5 Cs1 Mo1 O2 -51.2(2) 2_556 . . . ?
O10 Cs1 Mo1 O2 -172.9(3) 2 . . . ?
Mo3 Cs1 Mo1 O2 159.60(18) 2 . . . ?
O5 Cs1 Mo1 O3 -115.9(3) 1_464 . . . ?
O8 Cs1 Mo1 O3 -167.2(4) . . . . ?
O6 Cs1 Mo1 O3 18.2(3) 2 . . . ?
O9 Cs1 Mo1 O3 165.7(3) 2_455 . . . ?
O3 Cs1 Mo1 O3 69.5(3) 2 . . . ?
O7 Cs1 Mo1 O3 -55.7(3) 2_565 . . . ?
O4 Cs1 Mo1 O3 -6.8(3) . . . . ?
O9 Cs1 Mo1 O3 113.3(3) . . . . ?
O4 Cs1 Mo1 O3 64.8(3) 2 . . . ?
O5 Cs1 Mo1 O3 -122.0(3) 2_556 . . . ?
O10 Cs1 Mo1 O3 116.4(3) 2 . . . ?
Mo3 Cs1 Mo1 O3 88.9(2) 2 . . . ?
O5 Cs1 Mo1 Mo3 -92.1(3) 1_464 . . . ?
O8 Cs1 Mo1 Mo3 -143.4(4) . . . . ?
O6 Cs1 Mo1 Mo3 41.90(15) 2 . . . ?
O9 Cs1 Mo1 Mo3 -170.57(15) 2_455 . . . ?
O3 Cs1 Mo1 Mo3 93.25(17) 2 . . . ?
O7 Cs1 Mo1 Mo3 -31.94(15) 2_565 . . . ?
O4 Cs1 Mo1 Mo3 16.9(3) . . . . ?
O9 Cs1 Mo1 Mo3 137.06(15) . . . . ?
O4 Cs1 Mo1 Mo3 88.55(16) 2 . . . ?
O5 Cs1 Mo1 Mo3 -98.23(17) 2_556 . . . ?
O10 Cs1 Mo1 Mo3 140.1(2) 2 . . . ?
Mo3 Cs1 Mo1 Mo3 112.61(7) 2 . . . ?
O5 Cs1 Mo1 Mo1 -23.1(3) 1_464 . . 2_556 ?
O8 Cs1 Mo1 Mo1 -74.4(4) . . . 2_556 ?
O6 Cs1 Mo1 Mo1 110.95(15) 2 . . 2_556 ?
O9 Cs1 Mo1 Mo1 -101.52(17) 2_455 . . 2_556 ?
O3 Cs1 Mo1 Mo1 162.30(15) 2 . . 2_556 ?
O7 Cs1 Mo1 Mo1 37.10(16) 2_565 . . 2_556 ?
O4 Cs1 Mo1 Mo1 85.9(3) . . . 2_556 ?
O9 Cs1 Mo1 Mo1 -153.89(15) . . . 2_556 ?
O4 Cs1 Mo1 Mo1 157.60(14) 2 . . 2_556 ?
O5 Cs1 Mo1 Mo1 -29.19(15) 2_556 . . 2_556 ?
O10 Cs1 Mo1 Mo1 -150.9(2) 2 . . 2_556 ?
Mo3 Cs1 Mo1 Mo1 -178.34(5) 2 . . 2_556 ?
O5 Cs1 Mo1 K1 129.8(3) 1_464 . . 1_646 ?
O8 Cs1 Mo1 K1 78.5(4) . . . 1_646 ?
O6 Cs1 Mo1 K1 -96.15(19) 2 . . 1_646 ?
O9 Cs1 Mo1 K1 51.38(19) 2_455 . . 1_646 ?
O3 Cs1 Mo1 K1 -44.80(19) 2 . . 1_646 ?
O7 Cs1 Mo1 K1 -170.00(19) 2_565 . . 1_646 ?
O4 Cs1 Mo1 K1 -121.1(3) . . . 1_646 ?
O9 Cs1 Mo1 K1 -0.99(18) . . . 1_646 ?
O4 Cs1 Mo1 K1 -49.50(18) 2 . . 1_646 ?
O5 Cs1 Mo1 K1 123.71(19) 2_556 . . 1_646 ?
O10 Cs1 Mo1 K1 2.0(3) 2 . . 1_646 ?
Mo3 Cs1 Mo1 K1 -25.44(12) 2 . . 1_646 ?
O5 Cs1 Mo1 Cs1 -158.3(3) 1_464 . . 2 ?
O8 Cs1 Mo1 Cs1 150.4(4) . . . 2 ?
O6 Cs1 Mo1 Cs1 -24.24(14) 2 . . 2 ?
O9 Cs1 Mo1 Cs1 123.29(17) 2_455 . . 2 ?
O3 Cs1 Mo1 Cs1 27.11(14) 2 . . 2 ?
O7 Cs1 Mo1 Cs1 -98.09(17) 2_565 . . 2 ?
O4 Cs1 Mo1 Cs1 -49.2(3) . . . 2 ?
O9 Cs1 Mo1 Cs1 70.91(16) . . . 2 ?
O4 Cs1 Mo1 Cs1 22.41(13) 2 . . 2 ?
O5 Cs1 Mo1 Cs1 -164.38(14) 2_556 . . 2 ?
O10 Cs1 Mo1 Cs1 74.0(2) 2 . . 2 ?
Mo3 Cs1 Mo1 Cs1 46.47(4) 2 . . 2 ?
O5 Cs1 Mo1 K1 133.8(3) 1_464 . . 2_455 ?
O8 Cs1 Mo1 K1 82.5(4) . . . 2_455 ?
O6 Cs1 Mo1 K1 -92.20(15) 2 . . 2_455 ?
O9 Cs1 Mo1 K1 55.33(16) 2_455 . . 2_455 ?
O3 Cs1 Mo1 K1 -40.85(16) 2 . . 2_455 ?
O7 Cs1 Mo1 K1 -166.05(15) 2_565 . . 2_455 ?
O4 Cs1 Mo1 K1 -117.2(3) . . . 2_455 ?
O9 Cs1 Mo1 K1 2.96(14) . . . 2_455 ?
O4 Cs1 Mo1 K1 -45.55(15) 2 . . 2_455 ?
O5 Cs1 Mo1 K1 127.66(16) 2_556 . . 2_455 ?
O10 Cs1 Mo1 K1 6.0(2) 2 . . 2_455 ?
Mo3 Cs1 Mo1 K1 -21.49(5) 2 . . 2_455 ?
O8 Mo1 Mo3 O7 22.9(5) . . . . ?
O6 Mo1 Mo3 O7 152.6(4) . . . . ?
O2 Mo1 Mo3 O7 -93.7(4) 2_556 . . . ?
O4 Mo1 Mo3 O7 77.7(5) . . . . ?
O2 Mo1 Mo3 O7 -47.5(4) . . . . ?
O3 Mo1 Mo3 O7 -153.7(4) . . . . ?
Mo1 Mo1 Mo3 O7 -71.4(3) 2_556 . . . ?
K1 Mo1 Mo3 O7 -144.0(3) 1_646 . . . ?
Cs1 Mo1 Mo3 O7 53.8(3) . . . . ?
Cs1 Mo1 Mo3 O7 145.6(3) 2 . . . ?
K1 Mo1 Mo3 O7 131.6(3) 2_455 . . . ?
O8 Mo1 Mo3 O9 -106.0(5) . . . 2 ?
O6 Mo1 Mo3 O9 23.6(5) . . . 2 ?
O2 Mo1 Mo3 O9 137.3(4) 2_556 . . 2 ?
O4 Mo1 Mo3 O9 -51.3(5) . . . 2 ?
O2 Mo1 Mo3 O9 -176.5(4) . . . 2 ?
O3 Mo1 Mo3 O9 77.3(4) . . . 2 ?
Mo1 Mo1 Mo3 O9 159.6(3) 2_556 . . 2 ?
K1 Mo1 Mo3 O9 87.1(4) 1_646 . . 2 ?
Cs1 Mo1 Mo3 O9 -75.2(4) . . . 2 ?
Cs1 Mo1 Mo3 O9 16.6(3) 2 . . 2 ?
K1 Mo1 Mo3 O9 2.6(4) 2_455 . . 2 ?
O8 Mo1 Mo3 O4 -54.8(5) . . . . ?
O6 Mo1 Mo3 O4 74.9(5) . . . . ?
O2 Mo1 Mo3 O4 -171.4(4) 2_556 . . . ?
O2 Mo1 Mo3 O4 -125.2(5) . . . . ?
O3 Mo1 Mo3 O4 128.6(5) . . . . ?
Mo1 Mo1 Mo3 O4 -149.1(4) 2_556 . . . ?
K1 Mo1 Mo3 O4 138.3(4) 1_646 . . . ?
Cs1 Mo1 Mo3 O4 -23.9(4) . . . . ?
Cs1 Mo1 Mo3 O4 67.9(4) 2 . . . ?
K1 Mo1 Mo3 O4 53.9(4) 2_455 . . . ?
O8 Mo1 Mo3 O1 138.5(4) . . . . ?
O6 Mo1 Mo3 O1 -91.8(4) . . . . ?
O2 Mo1 Mo3 O1 21.9(3) 2_556 . . . ?
O4 Mo1 Mo3 O1 -166.7(4) . . . . ?
O2 Mo1 Mo3 O1 68.1(3) . . . . ?
O3 Mo1 Mo3 O1 -38.1(3) . . . . ?
Mo1 Mo1 Mo3 O1 44.1(2) 2_556 . . . ?
K1 Mo1 Mo3 O1 -28.4(2) 1_646 . . . ?
Cs1 Mo1 Mo3 O1 169.4(2) . . . . ?
Cs1 Mo1 Mo3 O1 -98.8(2) 2 . . . ?
K1 Mo1 Mo3 O1 -112.8(2) 2_455 . . . ?
O8 Mo1 Mo3 O3 176.6(4) . . . . ?
O6 Mo1 Mo3 O3 -53.8(4) . . . . ?
O2 Mo1 Mo3 O3 59.9(3) 2_556 . . . ?
O4 Mo1 Mo3 O3 -128.6(5) . . . . ?
O2 Mo1 Mo3 O3 106.2(4) . . . . ?
Mo1 Mo1 Mo3 O3 82.2(3) 2_556 . . . ?
K1 Mo1 Mo3 O3 9.7(2) 1_646 . . . ?
Cs1 Mo1 Mo3 O3 -152.5(2) . . . . ?
Cs1 Mo1 Mo3 O3 -60.8(3) 2 . . . ?
K1 Mo1 Mo3 O3 -74.8(3) 2_455 . . . ?
O8 Mo1 Mo3 O2 70.5(4) . . . . ?
O6 Mo1 Mo3 O2 -159.9(4) . . . . ?
O2 Mo1 Mo3 O2 -46.2(4) 2_556 . . . ?
O4 Mo1 Mo3 O2 125.2(5) . . . . ?
O3 Mo1 Mo3 O2 -106.2(4) . . . . ?
Mo1 Mo1 Mo3 O2 -23.9(2) 2_556 . . . ?
K1 Mo1 Mo3 O2 -96.4(3) 1_646 . . . ?
Cs1 Mo1 Mo3 O2 101.3(3) . . . . ?
Cs1 Mo1 Mo3 O2 -166.9(2) 2 . . . ?
K1 Mo1 Mo3 O2 179.1(3) 2_455 . . . ?
O8 Mo1 Mo3 K1 -43.2(3) . . . 1_655 ?
O6 Mo1 Mo3 K1 86.4(3) . . . 1_655 ?
O2 Mo1 Mo3 K1 -159.9(2) 2_556 . . 1_655 ?
O4 Mo1 Mo3 K1 11.5(4) . . . 1_655 ?
O2 Mo1 Mo3 K1 -113.7(3) . . . 1_655 ?
O3 Mo1 Mo3 K1 140.2(3) . . . 1_655 ?
Mo1 Mo1 Mo3 K1 -137.61(9) 2_556 . . 1_655 ?
K1 Mo1 Mo3 K1 149.88(9) 1_646 . . 1_655 ?
Cs1 Mo1 Mo3 K1 -12.36(6) . . . 1_655 ?
Cs1 Mo1 Mo3 K1 79.41(10) 2 . . 1_655 ?
K1 Mo1 Mo3 K1 65.41(13) 2_455 . . 1_655 ?
O8 Mo1 Mo3 Cs1 -122.6(3) . . . 2 ?
O6 Mo1 Mo3 Cs1 7.0(3) . . . 2 ?
O2 Mo1 Mo3 Cs1 120.7(2) 2_556 . . 2 ?
O4 Mo1 Mo3 Cs1 -67.9(4) . . . 2 ?
O2 Mo1 Mo3 Cs1 166.9(2) . . . 2 ?
O3 Mo1 Mo3 Cs1 60.8(3) . . . 2 ?
Mo1 Mo1 Mo3 Cs1 142.98(5) 2_556 . . 2 ?
K1 Mo1 Mo3 Cs1 70.47(11) 1_646 . . 2 ?
Cs1 Mo1 Mo3 Cs1 -91.77(10) . . . 2 ?
K1 Mo1 Mo3 Cs1 -14.00(6) 2_455 . . 2 ?
O8 Mo1 Mo3 K1 37.4(3) . . . 2_465 ?
O6 Mo1 Mo3 K1 167.0(3) . . . 2_465 ?
O2 Mo1 Mo3 K1 -79.3(2) 2_556 . . 2_465 ?
O4 Mo1 Mo3 K1 92.1(4) . . . 2_465 ?
O2 Mo1 Mo3 K1 -33.1(3) . . . 2_465 ?
O3 Mo1 Mo3 K1 -139.2(3) . . . 2_465 ?
Mo1 Mo1 Mo3 K1 -57.01(6) 2_556 . . 2_465 ?
K1 Mo1 Mo3 K1 -129.52(8) 1_646 . . 2_465 ?
Cs1 Mo1 Mo3 K1 68.24(9) . . . 2_465 ?
Cs1 Mo1 Mo3 K1 160.01(5) 2 . . 2_465 ?
K1 Mo1 Mo3 K1 146.01(10) 2_455 . . 2_465 ?
O8 Mo1 Mo3 Cs1 -130.7(3) . . . 1_655 ?
O6 Mo1 Mo3 Cs1 -1.1(3) . . . 1_655 ?
O2 Mo1 Mo3 Cs1 112.6(2) 2_556 . . 1_655 ?
O4 Mo1 Mo3 Cs1 -76.0(4) . . . 1_655 ?
O2 Mo1 Mo3 Cs1 158.8(3) . . . 1_655 ?
O3 Mo1 Mo3 Cs1 52.7(3) . . . 1_655 ?
Mo1 Mo1 Mo3 Cs1 134.91(8) 2_556 . . 1_655 ?
K1 Mo1 Mo3 Cs1 62.39(13) 1_646 . . 1_655 ?
Cs1 Mo1 Mo3 Cs1 -99.84(12) . . . 1_655 ?
Cs1 Mo1 Mo3 Cs1 -8.08(8) 2 . . 1_655 ?
K1 Mo1 Mo3 Cs1 -22.08(11) 2_455 . . 1_655 ?
O7 Mo3 O1 Mo2 -12.7(7) . . . 2_656 ?
O9 Mo3 O1 Mo2 91.5(7) 2 . . 2_656 ?
O4 Mo3 O1 Mo2 -153.4(6) . . . 2_656 ?
O3 Mo3 O1 Mo2 -168.6(7) . . . 2_656 ?
O2 Mo3 O1 Mo2 -98.1(6) . . . 2_656 ?
Mo1 Mo3 O1 Mo2 -139.0(6) . . . 2_656 ?
K1 Mo3 O1 Mo2 43.1(8) 1_655 . . 2_656 ?
Cs1 Mo3 O1 Mo2 149.9(6) 2 . . 2_656 ?
K1 Mo3 O1 Mo2 -57.5(7) 2_465 . . 2_656 ?
Cs1 Mo3 O1 Mo2 68.6(6) 1_655 . . 2_656 ?
O7 Mo3 O1 Mo2 162.4(3) . . . . ?
O9 Mo3 O1 Mo2 -93.5(4) 2 . . . ?
O4 Mo3 O1 Mo2 21.7(7) . . . . ?
O3 Mo3 O1 Mo2 6.5(3) . . . . ?
O2 Mo3 O1 Mo2 76.9(3) . . . . ?
Mo1 Mo3 O1 Mo2 36.0(3) . . . . ?
K1 Mo3 O1 Mo2 -141.81(17) 1_655 . . . ?
Cs1 Mo3 O1 Mo2 -35.1(3) 2 . . . ?
K1 Mo3 O1 Mo2 117.5(2) 2_465 . . . ?
Cs1 Mo3 O1 Mo2 -116.4(3) 1_655 . . . ?
O10 Mo2 O1 Mo3 88.9(4) . . . . ?
O5 Mo2 O1 Mo3 -100.1(6) . . . . ?
O3 Mo2 O1 Mo3 -7.7(3) . . . . ?
O1 Mo2 O1 Mo3 -177.0(5) 2_656 . . . ?
K1 Mo2 O1 Mo3 -39.6(4) 1_646 . . . ?
Cs1 Mo2 O1 Mo3 167.3(2) 1_646 . . . ?
Cs1 Mo2 O1 Mo3 30.1(3) 2 . . . ?
Cs1 Mo2 O1 Mo3 -116.9(3) 2_556 . . . ?
O10 Mo2 O1 Mo2 -94.0(4) . . . 2_656 ?
O5 Mo2 O1 Mo2 77.0(7) . . . 2_656 ?
O3 Mo2 O1 Mo2 169.4(4) . . . 2_656 ?
O1 Mo2 O1 Mo2 0.0 2_656 . . 2_656 ?
K1 Mo2 O1 Mo2 137.5(2) 1_646 . . 2_656 ?
Cs1 Mo2 O1 Mo2 -15.7(7) 1_646 . . 2_656 ?
Cs1 Mo2 O1 Mo2 -152.9(3) 2 . . 2_656 ?
Cs1 Mo2 O1 Mo2 60.1(3) 2_556 . . 2_656 ?
O8 Mo1 O2 Mo1 98.3(4) . . . 2_556 ?
O6 Mo1 O2 Mo1 -85.8(8) . . . 2_556 ?
O2 Mo1 O2 Mo1 0.0 2_556 . . 2_556 ?
O4 Mo1 O2 Mo1 -165.1(4) . . . 2_556 ?
O3 Mo1 O2 Mo1 -89.1(3) . . . 2_556 ?
Mo3 Mo1 O2 Mo1 -135.3(4) . . . 2_556 ?
K1 Mo1 O2 Mo1 -32.4(3) 1_646 . . 2_556 ?
Cs1 Mo1 O2 Mo1 145.3(3) . . . 2_556 ?
Cs1 Mo1 O2 Mo1 -122.3(2) 2 . . 2_556 ?
K1 Mo1 O2 Mo1 79(9) 2_455 . . 2_556 ?
O8 Mo1 O2 Mo3 -126.3(3) . . . . ?
O6 Mo1 O2 Mo3 49.6(8) . . . . ?
O2 Mo1 O2 Mo3 135.3(4) 2_556 . . . ?
O4 Mo1 O2 Mo3 -29.8(3) . . . . ?
O3 Mo1 O2 Mo3 46.2(2) . . . . ?
Mo1 Mo1 O2 Mo3 135.3(4) 2_556 . . . ?
K1 Mo1 O2 Mo3 102.91(19) 1_646 . . . ?
Cs1 Mo1 O2 Mo3 -79.3(2) . . . . ?
Cs1 Mo1 O2 Mo3 13.0(2) 2 . . . ?
K1 Mo1 O2 Mo3 -146(9) 2_455 . . . ?
O8 Mo1 O2 K1 -22.8(4) . . . 2_465 ?
O6 Mo1 O2 K1 153.1(7) . . . 2_465 ?
O2 Mo1 O2 K1 -121.1(5) 2_556 . . 2_465 ?
O4 Mo1 O2 K1 73.8(4) . . . 2_465 ?
O3 Mo1 O2 K1 149.8(4) . . . 2_465 ?
Mo3 Mo1 O2 K1 103.6(4) . . . 2_465 ?
Mo1 Mo1 O2 K1 -121.1(5) 2_556 . . 2_465 ?
K1 Mo1 O2 K1 -153.5(2) 1_646 . . 2_465 ?
Cs1 Mo1 O2 K1 24.2(3) . . . 2_465 ?
Cs1 Mo1 O2 K1 116.6(3) 2 . . 2_465 ?
K1 Mo1 O2 K1 -42(9) 2_455 . . 2_465 ?
O7 Mo3 O2 Mo1 -112.4(5) . . . 2_556 ?
O9 Mo3 O2 Mo1 121.4(14) 2 . . 2_556 ?
O4 Mo3 O2 Mo1 139.4(5) . . . 2_556 ?
O1 Mo3 O2 Mo1 -11.7(5) . . . 2_556 ?
O3 Mo3 O2 Mo1 58.2(5) . . . 2_556 ?
Mo1 Mo3 O2 Mo1 108.1(5) . . . 2_556 ?
K1 Mo3 O2 Mo1 -158.5(3) 1_655 . . 2_556 ?
Cs1 Mo3 O2 Mo1 95.2(4) 2 . . 2_556 ?
K1 Mo3 O2 Mo1 -123.6(6) 2_465 . . 2_556 ?
Cs1 Mo3 O2 Mo1 -47.1(8) 1_655 . . 2_556 ?
O7 Mo3 O2 Mo1 139.5(4) . . . . ?
O9 Mo3 O2 Mo1 13.2(16) 2 . . . ?
O4 Mo3 O2 Mo1 31.2(3) . . . . ?
O1 Mo3 O2 Mo1 -119.8(3) . . . . ?
O3 Mo3 O2 Mo1 -49.9(3) . . . . ?
K1 Mo3 O2 Mo1 93.4(2) 1_655 . . . ?
Cs1 Mo3 O2 Mo1 -12.9(2) 2 . . . ?
K1 Mo3 O2 Mo1 128.3(3) 2_465 . . . ?
Cs1 Mo3 O2 Mo1 -155.2(3) 1_655 . . . ?
O7 Mo3 O2 K1 11.2(3) . . . 2_465 ?
O9 Mo3 O2 K1 -115.0(14) 2 . . 2_465 ?
O4 Mo3 O2 K1 -97.0(3) . . . 2_465 ?
O1 Mo3 O2 K1 111.9(3) . . . 2_465 ?
O3 Mo3 O2 K1 -178.2(3) . . . 2_465 ?
Mo1 Mo3 O2 K1 -128.3(3) . . . 2_465 ?
K1 Mo3 O2 K1 -34.9(3) 1_655 . . 2_465 ?
Cs1 Mo3 O2 K1 -141.21(17) 2 . . 2_465 ?
Cs1 Mo3 O2 K1 76.5(5) 1_655 . . 2_465 ?
O10 Mo2 O3 Mo3 -97.6(4) . . . . ?
O5 Mo2 O3 Mo3 154.0(4) . . . . ?
O1 Mo2 O3 Mo3 24.2(6) 2_656 . . . ?
O1 Mo2 O3 Mo3 6.8(3) . . . . ?
K1 Mo2 O3 Mo3 161.7(4) 1_646 . . . ?
Cs1 Mo2 O3 Mo3 -170.84(11) 1_646 . . . ?
Cs1 Mo2 O3 Mo3 -102.1(4) 2 . . . ?
Cs1 Mo2 O3 Mo3 109.0(3) 2_556 . . . ?
O10 Mo2 O3 Mo1 151.1(7) . . . . ?
O5 Mo2 O3 Mo1 42.7(8) . . . . ?
O1 Mo2 O3 Mo1 -87.1(8) 2_656 . . . ?
O1 Mo2 O3 Mo1 -104.5(7) . . . . ?
K1 Mo2 O3 Mo1 50.4(6) 1_646 . . . ?
Cs1 Mo2 O3 Mo1 77.9(7) 1_646 . . . ?
Cs1 Mo2 O3 Mo1 146.6(9) 2 . . . ?
Cs1 Mo2 O3 Mo1 -2.3(8) 2_556 . . . ?
O10 Mo2 O3 Cs1 4.5(4) . . . 2 ?
O5 Mo2 O3 Cs1 -103.9(4) . . . 2 ?
O1 Mo2 O3 Cs1 126.3(4) 2_656 . . 2 ?
O1 Mo2 O3 Cs1 108.9(3) . . . 2 ?
K1 Mo2 O3 Cs1 -96.2(3) 1_646 . . 2 ?
Cs1 Mo2 O3 Cs1 -68.8(4) 1_646 . . 2 ?
Cs1 Mo2 O3 Cs1 -148.92(19) 2_556 . . 2 ?
O7 Mo3 O3 Mo2 -81.5(9) . . . . ?
O9 Mo3 O3 Mo2 87.4(4) 2 . . . ?
O4 Mo3 O3 Mo2 -179.0(4) . . . . ?
O1 Mo3 O3 Mo2 -7.7(3) . . . . ?
O2 Mo3 O3 Mo2 -104.5(4) . . . . ?
Mo1 Mo3 O3 Mo2 -150.1(4) . . . . ?
K1 Mo3 O3 Mo2 132.3(2) 1_655 . . . ?
Cs1 Mo3 O3 Mo2 119.7(4) 2 . . . ?
K1 Mo3 O3 Mo2 -105.8(3) 2_465 . . . ?
Cs1 Mo3 O3 Mo2 52.2(4) 1_655 . . . ?
O7 Mo3 O3 Mo1 68.6(9) . . . . ?
O9 Mo3 O3 Mo1 -122.5(3) 2 . . . ?
O4 Mo3 O3 Mo1 -28.9(3) . . . . ?
O1 Mo3 O3 Mo1 142.4(3) . . . . ?
O2 Mo3 O3 Mo1 45.6(2) . . . . ?
K1 Mo3 O3 Mo1 -77.6(3) 1_655 . . . ?
Cs1 Mo3 O3 Mo1 -90.2(2) 2 . . . ?
K1 Mo3 O3 Mo1 44.3(2) 2_465 . . . ?
Cs1 Mo3 O3 Mo1 -157.70(10) 1_655 . . . ?
O7 Mo3 O3 Cs1 158.8(8) . . . 2 ?
O9 Mo3 O3 Cs1 -32.3(3) 2 . . 2 ?
O4 Mo3 O3 Cs1 61.3(3) . . . 2 ?
O1 Mo3 O3 Cs1 -127.4(3) . . . 2 ?
O2 Mo3 O3 Cs1 135.8(3) . . . 2 ?
Mo1 Mo3 O3 Cs1 90.2(2) . . . 2 ?
K1 Mo3 O3 Cs1 12.6(4) 1_655 . . 2 ?
K1 Mo3 O3 Cs1 134.45(12) 2_465 . . 2 ?
Cs1 Mo3 O3 Cs1 -67.52(19) 1_655 . . 2 ?
O8 Mo1 O3 Mo2 104.1(15) . . . . ?
O6 Mo1 O3 Mo2 -110.2(7) . . . . ?
O2 Mo1 O3 Mo2 -7.8(7) 2_556 . . . ?
O4 Mo1 O3 Mo2 145.8(8) . . . . ?
O2 Mo1 O3 Mo2 68.4(7) . . . . ?
Mo3 Mo1 O3 Mo2 117.3(8) . . . . ?
Mo1 Mo1 O3 Mo2 33.0(6) 2_556 . . . ?
K1 Mo1 O3 Mo2 -53.0(7) 1_646 . . . ?
Cs1 Mo1 O3 Mo2 151.7(6) . . . . ?
Cs1 Mo1 O3 Mo2 -150.8(8) 2 . . . ?
K1 Mo1 O3 Mo2 -111.4(7) 2_455 . . . ?
O8 Mo1 O3 Mo3 -13.2(16) . . . . ?
O6 Mo1 O3 Mo3 132.5(3) . . . . ?
O2 Mo1 O3 Mo3 -125.1(3) 2_556 . . . ?
O4 Mo1 O3 Mo3 28.6(3) . . . . ?
O2 Mo1 O3 Mo3 -48.9(2) . . . . ?
Mo1 Mo1 O3 Mo3 -84.3(2) 2_556 . . . ?
K1 Mo1 O3 Mo3 -170.3(2) 1_646 . . . ?
Cs1 Mo1 O3 Mo3 34.4(3) . . . . ?
Cs1 Mo1 O3 Mo3 92.0(2) 2 . . . ?
K1 Mo1 O3 Mo3 131.36(17) 2_455 . . . ?
O8 Mo1 O3 Cs1 -105.2(15) . . . 2 ?
O6 Mo1 O3 Cs1 40.5(3) . . . 2 ?
O2 Mo1 O3 Cs1 143.0(3) 2_556 . . 2 ?
O4 Mo1 O3 Cs1 -63.4(3) . . . 2 ?
O2 Mo1 O3 Cs1 -140.9(3) . . . 2 ?
Mo3 Mo1 O3 Cs1 -92.0(2) . . . 2 ?
Mo1 Mo1 O3 Cs1 -176.27(18) 2_556 . . 2 ?
K1 Mo1 O3 Cs1 97.8(2) 1_646 . . 2 ?
Cs1 Mo1 O3 Cs1 -57.6(2) . . . 2 ?
K1 Mo1 O3 Cs1 39.40(19) 2_455 . . 2 ?
O7 Mo3 O4 Mo1 -117.1(4) . . . . ?
O9 Mo3 O4 Mo1 138.4(4) 2 . . . ?
O1 Mo3 O4 Mo1 22.7(7) . . . . ?
O3 Mo3 O4 Mo1 37.4(3) . . . . ?
O2 Mo3 O4 Mo1 -37.5(3) . . . . ?
K1 Mo3 O4 Mo1 -169.4(3) 1_655 . . . ?
Cs1 Mo3 O4 Mo1 93.0(3) 2 . . . ?
K1 Mo3 O4 Mo1 -80.5(3) 2_465 . . . ?
Cs1 Mo3 O4 Mo1 145.67(19) 1_655 . . . ?
O7 Mo3 O4 Cs1 9.1(6) . . . . ?
O9 Mo3 O4 Cs1 -95.4(6) 2 . . . ?
O1 Mo3 O4 Cs1 148.8(4) . . . . ?
O3 Mo3 O4 Cs1 163.6(6) . . . . ?
O2 Mo3 O4 Cs1 88.6(5) . . . . ?
Mo1 Mo3 O4 Cs1 126.1(7) . . . . ?
K1 Mo3 O4 Cs1 -43.3(5) 1_655 . . . ?
Cs1 Mo3 O4 Cs1 -140.9(6) 2 . . . ?
K1 Mo3 O4 Cs1 45.7(5) 2_465 . . . ?
Cs1 Mo3 O4 Cs1 -88.2(5) 1_655 . . . ?
O7 Mo3 O4 Cs1 149.9(3) . . . 2 ?
O9 Mo3 O4 Cs1 45.4(3) 2 . . 2 ?
O1 Mo3 O4 Cs1 -70.4(5) . . . 2 ?
O3 Mo3 O4 Cs1 -55.6(2) . . . 2 ?
O2 Mo3 O4 Cs1 -130.5(3) . . . 2 ?
Mo1 Mo3 O4 Cs1 -93.0(3) . . . 2 ?
K1 Mo3 O4 Cs1 97.56(16) 1_655 . . 2 ?
K1 Mo3 O4 Cs1 -173.47(16) 2_465 . . 2 ?
Cs1 Mo3 O4 Cs1 52.7(3) 1_655 . . 2 ?
O8 Mo1 O4 Mo3 135.7(4) . . . . ?
O6 Mo1 O4 Mo3 -116.3(4) . . . . ?
O2 Mo1 O4 Mo3 14.0(7) 2_556 . . . ?
O2 Mo1 O4 Mo3 39.4(3) . . . . ?
O3 Mo1 O4 Mo3 -35.8(3) . . . . ?
Mo1 Mo1 O4 Mo3 30.9(4) 2_556 . . . ?
K1 Mo1 O4 Mo3 -60.8(5) 1_646 . . . ?
Cs1 Mo1 O4 Mo3 150.0(5) . . . . ?
Cs1 Mo1 O4 Mo3 -93.1(4) 2 . . . ?
K1 Mo1 O4 Mo3 -141.7(3) 2_455 . . . ?
O8 Mo1 O4 Cs1 -14.3(3) . . . . ?
O6 Mo1 O4 Cs1 93.7(3) . . . . ?
O2 Mo1 O4 Cs1 -136.0(4) 2_556 . . . ?
O2 Mo1 O4 Cs1 -110.6(3) . . . . ?
O3 Mo1 O4 Cs1 174.1(3) . . . . ?
Mo3 Mo1 O4 Cs1 -150.0(5) . . . . ?
Mo1 Mo1 O4 Cs1 -119.15(15) 2_556 . . . ?
K1 Mo1 O4 Cs1 149.13(14) 1_646 . . . ?
Cs1 Mo1 O4 Cs1 116.8(3) 2 . . . ?
K1 Mo1 O4 Cs1 68.3(2) 2_455 . . . ?
O8 Mo1 O4 Cs1 -131.2(3) . . . 2 ?
O6 Mo1 O4 Cs1 -23.1(3) . . . 2 ?
O2 Mo1 O4 Cs1 107.2(5) 2_556 . . 2 ?
O2 Mo1 O4 Cs1 132.5(3) . . . 2 ?
O3 Mo1 O4 Cs1 57.3(2) . . . 2 ?
Mo3 Mo1 O4 Cs1 93.1(4) . . . 2 ?
Mo1 Mo1 O4 Cs1 124.02(14) 2_556 . . 2 ?
K1 Mo1 O4 Cs1 32.3(3) 1_646 . . 2 ?
Cs1 Mo1 O4 Cs1 -116.8(3) . . . 2 ?
K1 Mo1 O4 Cs1 -48.6(2) 2_455 . . 2 ?
O5 Cs1 O4 Mo3 -14.3(7) 1_464 . . . ?
O8 Cs1 O4 Mo3 -119.3(6) . . . . ?
O6 Cs1 O4 Mo3 77.7(5) 2 . . . ?
O9 Cs1 O4 Mo3 -138.6(5) 2_455 . . . ?
O3 Cs1 O4 Mo3 116.2(5) 2 . . . ?
O7 Cs1 O4 Mo3 -2.0(5) 2_565 . . . ?
O9 Cs1 O4 Mo3 172.5(5) . . . . ?
O4 Cs1 O4 Mo3 135.3(7) 2 . . . ?
O5 Cs1 O4 Mo3 -73.1(5) 2_556 . . . ?
O10 Cs1 O4 Mo3 123.9(5) 2 . . . ?
Mo3 Cs1 O4 Mo3 147.3(5) 2 . . . ?
O5 Cs1 O4 Mo1 115.0(3) 1_464 . . . ?
O8 Cs1 O4 Mo1 9.9(2) . . . . ?
O6 Cs1 O4 Mo1 -153.1(3) 2 . . . ?
O9 Cs1 O4 Mo1 -9.4(4) 2_455 . . . ?
O3 Cs1 O4 Mo1 -114.6(3) 2 . . . ?
O7 Cs1 O4 Mo1 127.2(3) 2_565 . . . ?
O9 Cs1 O4 Mo1 -58.2(3) . . . . ?
O4 Cs1 O4 Mo1 -95.5(3) 2 . . . ?
O5 Cs1 O4 Mo1 56.1(3) 2_556 . . . ?
O10 Cs1 O4 Mo1 -106.9(4) 2 . . . ?
Mo3 Cs1 O4 Mo1 -83.5(2) 2 . . . ?
O5 Cs1 O4 Cs1 -149.5(3) 1_464 . . 2 ?
O8 Cs1 O4 Cs1 105.4(3) . . . 2 ?
O6 Cs1 O4 Cs1 -57.6(2) 2 . . 2 ?
O9 Cs1 O4 Cs1 86.1(3) 2_455 . . 2 ?
O3 Cs1 O4 Cs1 -19.0(3) 2 . . 2 ?
O7 Cs1 O4 Cs1 -137.3(3) 2_565 . . 2 ?
O9 Cs1 O4 Cs1 37.3(2) . . . 2 ?
O4 Cs1 O4 Cs1 0.0 2 . . 2 ?
O5 Cs1 O4 Cs1 151.6(2) 2_556 . . 2 ?
O10 Cs1 O4 Cs1 -11.3(5) 2 . . 2 ?
Mo3 Cs1 O4 Cs1 12.07(19) 2 . . 2 ?
O10 Mo2 O5 K1 -94.5(5) . . . 1_646 ?
O3 Mo2 O5 K1 10.9(5) . . . 1_646 ?
O1 Mo2 O5 K1 163.9(4) 2_656 . . 1_646 ?
O1 Mo2 O5 K1 94.4(6) . . . 1_646 ?
Cs1 Mo2 O5 K1 -121.7(6) 1_646 . . 1_646 ?
Cs1 Mo2 O5 K1 -31.1(4) 2 . . 1_646 ?
Cs1 Mo2 O5 K1 118.3(6) 2_556 . . 1_646 ?
O10 Mo2 O5 Cs1 27.2(5) . . . 1_646 ?
O3 Mo2 O5 Cs1 132.6(4) . . . 1_646 ?
O1 Mo2 O5 Cs1 -74.4(4) 2_656 . . 1_646 ?
O1 Mo2 O5 Cs1 -143.8(4) . . . 1_646 ?
K1 Mo2 O5 Cs1 121.7(6) 1_646 . . 1_646 ?
Cs1 Mo2 O5 Cs1 90.6(4) 2 . . 1_646 ?
Cs1 Mo2 O5 Cs1 -120.0(6) 2_556 . . 1_646 ?
O10 Mo2 O5 Cs1 147.2(4) . . . 2_556 ?
O3 Mo2 O5 Cs1 -107.4(4) . . . 2_556 ?
O1 Mo2 O5 Cs1 45.5(4) 2_656 . . 2_556 ?
O1 Mo2 O5 Cs1 -23.9(8) . . . 2_556 ?
K1 Mo2 O5 Cs1 -118.3(5) 1_646 . . 2_556 ?
Cs1 Mo2 O5 Cs1 120.0(6) 1_646 . . 2_556 ?
Cs1 Mo2 O5 Cs1 -149.4(2) 2 . . 2_556 ?
O8 Mo1 O6 K1 -4.9(7) . . . 2_455 ?
O2 Mo1 O6 K1 99.3(6) 2_556 . . 2_455 ?
O4 Mo1 O6 K1 -107.5(6) . . . 2_455 ?
O2 Mo1 O6 K1 179.3(4) . . . 2_455 ?
O3 Mo1 O6 K1 -177.6(6) . . . 2_455 ?
Mo3 Mo1 O6 K1 -142.4(5) . . . 2_455 ?
Mo1 Mo1 O6 K1 123.6(5) 2_556 . . 2_455 ?
K1 Mo1 O6 K1 115.8(6) 1_646 . . 2_455 ?
Cs1 Mo1 O6 K1 -52.5(6) . . . 2_455 ?
Cs1 Mo1 O6 K1 -133.9(7) 2 . . 2_455 ?
O8 Mo1 O6 Cs1 128.9(3) . . . 2 ?
O2 Mo1 O6 Cs1 -126.9(3) 2_556 . . 2 ?
O4 Mo1 O6 Cs1 26.4(4) . . . 2 ?
O2 Mo1 O6 Cs1 -46.9(9) . . . 2 ?
O3 Mo1 O6 Cs1 -43.7(3) . . . 2 ?
Mo3 Mo1 O6 Cs1 -8.5(4) . . . 2 ?
Mo1 Mo1 O6 Cs1 -102.6(3) 2_556 . . 2 ?
K1 Mo1 O6 Cs1 -110.3(3) 1_646 . . 2 ?
Cs1 Mo1 O6 Cs1 81.4(3) . . . 2 ?
K1 Mo1 O6 Cs1 133.9(7) 2_455 . . 2 ?
O8 Mo1 O6 K1 -120.7(3) . . . 1_646 ?
O2 Mo1 O6 K1 -16.5(3) 2_556 . . 1_646 ?
O4 Mo1 O6 K1 136.7(3) . . . 1_646 ?
O2 Mo1 O6 K1 63.5(8) . . . 1_646 ?
O3 Mo1 O6 K1 66.6(2) . . . 1_646 ?
Mo3 Mo1 O6 K1 101.8(2) . . . 1_646 ?
Mo1 Mo1 O6 K1 7.8(5) 2_556 . . 1_646 ?
Cs1 Mo1 O6 K1 -168.30(13) . . . 1_646 ?
Cs1 Mo1 O6 K1 110.3(3) 2 . . 1_646 ?
K1 Mo1 O6 K1 -115.8(6) 2_455 . . 1_646 ?
O9 Mo3 O7 K1 158.3(4) 2 . . 2_465 ?
O4 Mo3 O7 K1 58.1(4) . . . 2_465 ?
O1 Mo3 O7 K1 -100.3(4) . . . 2_465 ?
O3 Mo3 O7 K1 -32.8(10) . . . 2_465 ?
O2 Mo3 O7 K1 -11.0(3) . . . 2_465 ?
Mo1 Mo3 O7 K1 20.5(5) . . . 2_465 ?
K1 Mo3 O7 K1 124.4(4) 1_655 . . 2_465 ?
Cs1 Mo3 O7 K1 113.3(4) 2 . . 2_465 ?
Cs1 Mo3 O7 K1 -170.8(3) 1_655 . . 2_465 ?
O9 Mo3 O7 K1 33.9(4) 2 . . 1_655 ?
O4 Mo3 O7 K1 -66.3(3) . . . 1_655 ?
O1 Mo3 O7 K1 135.2(3) . . . 1_655 ?
O3 Mo3 O7 K1 -157.2(7) . . . 1_655 ?
O2 Mo3 O7 K1 -135.4(3) . . . 1_655 ?
Mo1 Mo3 O7 K1 -103.9(2) . . . 1_655 ?
Cs1 Mo3 O7 K1 -11.1(6) 2 . . 1_655 ?
K1 Mo3 O7 K1 -124.4(4) 2_465 . . 1_655 ?
Cs1 Mo3 O7 K1 64.77(18) 1_655 . . 1_655 ?
O9 Mo3 O7 Cs1 -75.3(6) 2 . . 2_565 ?
O4 Mo3 O7 Cs1 -175.5(5) . . . 2_565 ?
O1 Mo3 O7 Cs1 26.1(6) . . . 2_565 ?
O3 Mo3 O7 Cs1 93.6(9) . . . 2_565 ?
O2 Mo3 O7 Cs1 115.4(6) . . . 2_565 ?
Mo1 Mo3 O7 Cs1 146.9(4) . . . 2_565 ?
K1 Mo3 O7 Cs1 -109.1(6) 1_655 . . 2_565 ?
Cs1 Mo3 O7 Cs1 -120.3(5) 2 . . 2_565 ?
K1 Mo3 O7 Cs1 126.4(8) 2_465 . . 2_565 ?
Cs1 Mo3 O7 Cs1 -44.4(5) 1_655 . . 2_565 ?
O6 Mo1 O8 Cs1 -88.6(4) . . . . ?
O2 Mo1 O8 Cs1 166.0(3) 2_556 . . . ?
O4 Mo1 O8 Cs1 16.0(4) . . . . ?
O2 Mo1 O8 Cs1 89.7(3) . . . . ?
O3 Mo1 O8 Cs1 55.8(16) . . . . ?
Mo3 Mo1 O8 Cs1 44.7(4) . . . . ?
Mo1 Mo1 O8 Cs1 123.9(3) 2_556 . . . ?
K1 Mo1 O8 Cs1 -150.01(14) 1_646 . . . ?
Cs1 Mo1 O8 Cs1 -39.6(5) 2 . . . ?
K1 Mo1 O8 Cs1 -90.7(3) 2_455 . . . ?
O5 Cs1 O8 Mo1 -146.1(3) 1_464 . . . ?
O6 Cs1 O8 Mo1 6.1(5) 2 . . . ?
O9 Cs1 O8 Mo1 152.5(4) 2_455 . . . ?
O3 Cs1 O8 Mo1 69.9(4) 2 . . . ?
O7 Cs1 O8 Mo1 -70.2(4) 2_565 . . . ?
O4 Cs1 O8 Mo1 -12.1(3) . . . . ?
O9 Cs1 O8 Mo1 94.9(4) . . . . ?
O4 Cs1 O8 Mo1 47.9(4) 2 . . . ?
O5 Cs1 O8 Mo1 -122.2(5) 2_556 . . . ?
O10 Cs1 O8 Mo1 129.9(3) 2 . . . ?
Mo3 Cs1 O8 Mo1 75.9(4) 2 . . . ?
O5 Cs1 O9 Mo3 103.7(4) 1_464 . . 2 ?
O8 Cs1 O9 Mo3 -131.1(4) . . . 2 ?
O6 Cs1 O9 Mo3 -12.3(4) 2 . . 2 ?
O9 Cs1 O9 Mo3 144.5(6) 2_455 . . 2 ?
O3 Cs1 O9 Mo3 24.9(3) 2 . . 2 ?
O7 Cs1 O9 Mo3 -61.8(9) 2_565 . . 2 ?
O4 Cs1 O9 Mo3 -81.1(4) . . . 2 ?
O4 Cs1 O9 Mo3 -33.5(3) 2 . . 2 ?
O5 Cs1 O9 Mo3 -161.2(3) 2_556 . . 2 ?
O10 Cs1 O9 Mo3 75.3(3) 2 . . 2 ?
O5 Cs1 O9 K1 -154.3(3) 1_464 . . 2_455 ?
O8 Cs1 O9 K1 -29.1(3) . . . 2_455 ?
O6 Cs1 O9 K1 89.8(3) 2 . . 2_455 ?
O9 Cs1 O9 K1 -113.5(4) 2_455 . . 2_455 ?
O3 Cs1 O9 K1 127.0(4) 2 . . 2_455 ?
O7 Cs1 O9 K1 40.2(9) 2_565 . . 2_455 ?
O4 Cs1 O9 K1 21.0(3) . . . 2_455 ?
O4 Cs1 O9 K1 68.5(3) 2 . . 2_455 ?
O5 Cs1 O9 K1 -59.2(3) 2_556 . . 2_455 ?
O10 Cs1 O9 K1 177.3(3) 2 . . 2_455 ?
Mo3 Cs1 O9 K1 102.0(5) 2 . . 2_455 ?
O5 Cs1 O9 Cs1 -40.8(4) 1_464 . . 2_455 ?
O8 Cs1 O9 Cs1 84.4(3) . . . 2_455 ?
O6 Cs1 O9 Cs1 -156.8(3) 2 . . 2_455 ?
O9 Cs1 O9 Cs1 0.0 2_455 . . 2_455 ?
O3 Cs1 O9 Cs1 -119.6(4) 2 . . 2_455 ?
O7 Cs1 O9 Cs1 153.7(6) 2_565 . . 2_455 ?
O4 Cs1 O9 Cs1 134.4(3) . . . 2_455 ?
O4 Cs1 O9 Cs1 -178.0(4) 2 . . 2_455 ?
O5 Cs1 O9 Cs1 54.3(4) 2_556 . . 2_455 ?
O10 Cs1 O9 Cs1 -69.2(3) 2 . . 2_455 ?
Mo3 Cs1 O9 Cs1 -144.5(6) 2 . . 2_455 ?
O5 Mo2 O10 K1 170(19) . . . 2 ?
O3 Mo2 O10 K1 61(19) . . . 2 ?
O1 Mo2 O10 K1 -89(19) 2_656 . . 2 ?
O1 Mo2 O10 K1 -15(19) . . . 2 ?
K1 Mo2 O10 K1 129(19) 1_646 . . 2 ?
Cs1 Mo2 O10 K1 -173(19) 1_646 . . 2 ?
Cs1 Mo2 O10 K1 64(19) 2 . . 2 ?
Cs1 Mo2 O10 K1 -157(19) 2_556 . . 2 ?
O5 Mo2 O10 Cs1 105.1(3) . . . 2 ?
O3 Mo2 O10 Cs1 -3.3(3) . . . 2 ?
O1 Mo2 O10 Cs1 -153.1(2) 2_656 . . 2 ?
O1 Mo2 O10 Cs1 -79.7(3) . . . 2 ?
K1 Mo2 O10 Cs1 64.1(2) 1_646 . . 2 ?
Cs1 Mo2 O10 Cs1 122.7(2) 1_646 . . 2 ?
Cs1 Mo2 O10 Cs1 138.6(2) 2_556 . . 2 ?

_diffrn_measured_fraction_theta_max 0.963
_diffrn_reflns_theta_full        27.43
_diffrn_measured_fraction_theta_full 0.963
_refine_diff_density_max         1.584
_refine_diff_density_min         -1.683
_refine_diff_density_rms         0.346
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_123
_database_code_depnum_ccdc_archive 'CCDC 1821288'
_audit_update_record             
;
2018-02-01 deposited with the CCDC.
2018-05-10 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
; 
 ? 
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'Cs Li Mo3 O10'
_chemical_formula_weight         587.67

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Li Li -0.0003 0.0001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           Orthorhombic
_symmetry_space_group_name_H-M   Pnma

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-x, y+1/2, -z'
'x+1/2, -y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, y, -z-1/2'
'x, -y-1/2, z'
'-x-1/2, y-1/2, z-1/2'

_cell_length_a                   8.652(2)
_cell_length_b                   7.5688(18)
_cell_length_c                   13.895(3)
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_volume                     909.9(4)
_cell_formula_units_Z            4
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    1930
_cell_measurement_theta_min      2.77
_cell_measurement_theta_max      27.34

_exptl_crystal_description       block
_exptl_crystal_colour            colorless
_exptl_crystal_size_max          0.15
_exptl_crystal_size_mid          0.103
_exptl_crystal_size_min          0.071
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    4.290
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1056
_exptl_absorpt_coefficient_mu    8.048
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_correction_T_min  0.6436
_exptl_absorpt_correction_T_max  0.8616
_exptl_absorpt_process_details   ?

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            5344
_diffrn_reflns_av_R_equivalents  0.0326
_diffrn_reflns_av_sigmaI/netI    0.0271
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_theta_min         2.77
_diffrn_reflns_theta_max         27.50
_reflns_number_total             1126
_reflns_number_gt                982
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0116P)²+2.0404P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   ?
_refine_ls_hydrogen_treatment    ?
_refine_ls_extinction_method     SHELXL
_refine_ls_extinction_coef       0.00284(13)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_number_reflns         1126
_refine_ls_number_parameters     80
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0264
_refine_ls_R_factor_gt           0.0208
_refine_ls_wR_factor_ref         0.0443
_refine_ls_wR_factor_gt          0.0394
_refine_ls_goodness_of_fit_ref   1.087
_refine_ls_restrained_S_all      1.087
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Li1 Li 0.0541(12) 0.2500 0.1603(8) 0.029(3) Uani 1 2 d S . .
Cs1 Cs 0.60001(4) 0.2500 0.60135(3) 0.02072(12) Uani 1 2 d S . .
Mo1 Mo 0.17439(5) 0.2500 0.40489(3) 0.00920(12) Uani 1 2 d S . .
Mo2 Mo 0.13187(4) -0.00008(4) 0.59909(2) 0.00911(10) Uani 1 1 d . . .
O1 O 0.1170(3) 0.0127(3) 0.43864(19) 0.0109(5) Uani 1 1 d . . .
O2 O 0.1355(4) 0.2500 0.5660(3) 0.0134(8) Uani 1 2 d S . .
O3 O 0.0796(4) -0.2500 0.5837(3) 0.0114(8) Uani 1 2 d S . .
O4 O 0.1536(4) 0.2500 0.2829(3) 0.0157(8) Uani 1 2 d S . .
O5 O 0.3720(4) 0.2500 0.4224(3) 0.0167(8) Uani 1 2 d S . .
O6 O 0.3270(3) -0.0444(4) 0.5964(2) 0.0166(6) Uani 1 1 d . . .
O7 O 0.0899(3) 0.0258(4) 0.7172(2) 0.0197(6) Uani 1 1 d . . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Li1 O4 1.909(11) . ?
Li1 O5 1.950(11) 6_556 ?
Li1 O6 2.066(8) 8_665 ?
Li1 O6 2.066(8) 2_554 ?
Li1 Cs1 3.657(11) 6_556 ?
Li1 Cs1 4.095(4) 2_554 ?
Li1 Cs1 4.095(4) 2_564 ?
Cs1 O7 3.040(3) 4_556 ?
Cs1 O7 3.040(3) 6_657 ?
Cs1 O5 3.174(4) . ?
Cs1 O1 3.203(2) 3_656 ?
Cs1 O1 3.203(2) 5_656 ?
Cs1 O6 3.220(3) 5_656 ?
Cs1 O6 3.220(3) 3_656 ?
Cs1 O6 3.248(3) . ?
Cs1 O6 3.248(3) 7_565 ?
Cs1 Li1 3.657(11) 6_656 ?
Cs1 O3 3.781(4) 5_656 ?
Cs1 O5 3.8065(10) 5_656 ?
Mo1 O4 1.705(4) . ?
Mo1 O5 1.727(4) . ?
Mo1 O1 1.922(2) . ?
Mo1 O1 1.922(2) 7_565 ?
Mo1 O3 2.203(4) 5_556 ?
Mo1 O2 2.264(4) . ?
Mo1 Cs1 4.2590(9) 5_666 ?
Mo1 Cs1 4.2590(9) 5_656 ?
Mo2 O7 1.693(3) . ?
Mo2 O6 1.721(3) . ?
Mo2 O2 1.9482(11) . ?
Mo2 O3 1.9567(11) . ?
Mo2 O1 2.218(3) 5_556 ?
Mo2 O1 2.235(3) . ?
Mo2 Cs1 4.0885(7) 5_656 ?
O1 Mo2 2.218(3) 5_556 ?
O1 Cs1 3.203(2) 5_656 ?
O2 Mo2 1.9482(11) 7_565 ?
O3 Mo2 1.9567(11) 7 ?
O3 Mo1 2.203(4) 5_556 ?
O3 Cs1 3.781(4) 5_656 ?
O5 Li1 1.950(11) 6_656 ?
O5 Cs1 3.8065(10) 5_656 ?
O5 Cs1 3.8065(10) 5_666 ?
O6 Li1 2.066(8) 2 ?
O6 Cs1 3.220(3) 5_656 ?
O7 Cs1 3.040(3) 6_557 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O4 Li1 O5 152.9(6) . 6_556 ?
O4 Li1 O6 99.1(4) . 8_665 ?
O5 Li1 O6 98.6(4) 6_556 8_665 ?
O4 Li1 O6 99.1(4) . 2_554 ?
O5 Li1 O6 98.6(4) 6_556 2_554 ?
O6 Li1 O6 97.7(5) 8_665 2_554 ?
O4 Li1 Cs1 146.9(5) . 6_556 ?
O5 Li1 Cs1 60.1(3) 6_556 6_556 ?
O6 Li1 Cs1 61.2(3) 8_665 6_556 ?
O6 Li1 Cs1 61.2(3) 2_554 6_556 ?
O4 Li1 Cs1 108.99(16) . 2_554 ?
O5 Li1 Cs1 67.61(13) 6_556 2_554 ?
O6 Li1 Cs1 140.6(4) 8_665 2_554 ?
O6 Li1 Cs1 51.69(13) 2_554 2_554 ?
Cs1 Li1 Cs1 80.59(15) 6_556 2_554 ?
O4 Li1 Cs1 108.99(16) . 2_564 ?
O5 Li1 Cs1 67.61(13) 6_556 2_564 ?
O6 Li1 Cs1 51.69(13) 8_665 2_564 ?
O6 Li1 Cs1 140.6(4) 2_554 2_564 ?
Cs1 Li1 Cs1 80.59(15) 6_556 2_564 ?
Cs1 Li1 Cs1 135.1(3) 2_554 2_564 ?
O7 Cs1 O7 67.86(11) 4_556 6_657 ?
O7 Cs1 O5 129.17(7) 4_556 . ?
O7 Cs1 O5 129.17(7) 6_657 . ?
O7 Cs1 O1 79.60(7) 4_556 3_656 ?
O7 Cs1 O1 120.83(7) 6_657 3_656 ?
O5 Cs1 O1 109.84(7) . 3_656 ?
O7 Cs1 O1 120.83(7) 4_556 5_656 ?
O7 Cs1 O1 79.60(7) 6_657 5_656 ?
O5 Cs1 O1 109.84(7) . 5_656 ?
O1 Cs1 O1 76.75(9) 3_656 5_656 ?
O7 Cs1 O6 169.39(7) 4_556 5_656 ?
O7 Cs1 O6 116.32(7) 6_657 5_656 ?
O5 Cs1 O6 56.88(7) . 5_656 ?
O1 Cs1 O6 90.12(7) 3_656 5_656 ?
O1 Cs1 O6 53.27(7) 5_656 5_656 ?
O7 Cs1 O6 116.32(7) 4_556 3_656 ?
O7 Cs1 O6 169.39(7) 6_657 3_656 ?
O5 Cs1 O6 56.88(7) . 3_656 ?
O1 Cs1 O6 53.27(7) 3_656 3_656 ?
O1 Cs1 O6 90.12(7) 5_656 3_656 ?
O6 Cs1 O6 57.80(10) 5_656 3_656 ?
O7 Cs1 O6 112.30(7) 4_556 . ?
O7 Cs1 O6 67.28(7) 6_657 . ?
O5 Cs1 O6 62.05(7) . . ?
O1 Cs1 O6 168.02(7) 3_656 . ?
O1 Cs1 O6 97.27(7) 5_656 . ?
O6 Cs1 O6 78.06(8) 5_656 . ?
O6 Cs1 O6 117.14(4) 3_656 . ?
O7 Cs1 O6 67.28(7) 4_556 7_565 ?
O7 Cs1 O6 112.30(7) 6_657 7_565 ?
O5 Cs1 O6 62.05(7) . 7_565 ?
O1 Cs1 O6 97.27(7) 3_656 7_565 ?
O1 Cs1 O6 168.02(7) 5_656 7_565 ?
O6 Cs1 O6 117.14(4) 5_656 7_565 ?
O6 Cs1 O6 78.06(8) 3_656 7_565 ?
O6 Cs1 O6 86.62(10) . 7_565 ?
O7 Cs1 Li1 145.20(6) 4_556 6_656 ?
O7 Cs1 Li1 145.20(6) 6_657 6_656 ?
O5 Cs1 Li1 32.19(18) . 6_656 ?
O1 Cs1 Li1 84.87(14) 3_656 6_656 ?
O1 Cs1 Li1 84.87(14) 5_656 6_656 ?
O6 Cs1 Li1 34.23(10) 5_656 6_656 ?
O6 Cs1 Li1 34.23(10) 3_656 6_656 ?
O6 Cs1 Li1 84.25(13) . 6_656 ?
O6 Cs1 Li1 84.25(13) 7_565 6_656 ?
O7 Cs1 O3 125.81(7) 4_556 5_656 ?
O7 Cs1 O3 125.81(7) 6_657 5_656 ?
O5 Cs1 O3 85.59(9) . 5_656 ?
O1 Cs1 O3 47.27(6) 3_656 5_656 ?
O1 Cs1 O3 47.27(6) 5_656 5_656 ?
O6 Cs1 O3 43.61(6) 5_656 5_656 ?
O6 Cs1 O3 43.61(6) 3_656 5_656 ?
O6 Cs1 O3 121.26(6) . 5_656 ?
O6 Cs1 O3 121.26(6) 7_565 5_656 ?
Li1 Cs1 O3 53.39(17) 6_656 5_656 ?
O7 Cs1 O5 128.96(8) 4_556 5_656 ?
O7 Cs1 O5 61.24(8) 6_657 5_656 ?
O5 Cs1 O5 88.37(6) . 5_656 ?
O1 Cs1 O5 123.61(7) 3_656 5_656 ?
O1 Cs1 O5 47.08(7) 5_656 5_656 ?
O6 Cs1 O5 55.45(8) 5_656 5_656 ?
O6 Cs1 O5 113.20(8) 3_656 5_656 ?
O6 Cs1 O5 50.39(7) . 5_656 ?
O6 Cs1 O5 136.59(7) 7_565 5_656 ?
Li1 Cs1 O5 85.45(6) 6_656 5_656 ?
O3 Cs1 O5 83.93(6) 5_656 5_656 ?
O4 Mo1 O5 104.16(18) . . ?
O4 Mo1 O1 102.45(9) . . ?
O5 Mo1 O1 102.80(8) . . ?
O4 Mo1 O1 102.45(9) . 7_565 ?
O5 Mo1 O1 102.80(9) . 7_565 ?
O1 Mo1 O1 138.34(15) . 7_565 ?
O4 Mo1 O3 88.09(16) . 5_556 ?
O5 Mo1 O3 167.75(17) . 5_556 ?
O1 Mo1 O3 74.01(8) . 5_556 ?
O1 Mo1 O3 74.01(8) 7_565 5_556 ?
O4 Mo1 O2 165.42(16) . . ?
O5 Mo1 O2 90.42(17) . . ?
O1 Mo1 O2 73.75(8) . . ?
O1 Mo1 O2 73.75(8) 7_565 . ?
O3 Mo1 O2 77.33(14) 5_556 . ?
O4 Mo1 Cs1 91.61(6) . 5_666 ?
O5 Mo1 Cs1 63.203(17) . 5_666 ?
O1 Mo1 Cs1 162.55(8) . 5_666 ?
O1 Mo1 Cs1 45.01(8) 7_565 5_666 ?
O3 Mo1 Cs1 117.294(11) 5_556 5_666 ?
O2 Mo1 Cs1 95.06(4) . 5_666 ?
O4 Mo1 Cs1 91.61(6) . 5_656 ?
O5 Mo1 Cs1 63.204(17) . 5_656 ?
O1 Mo1 Cs1 45.01(8) . 5_656 ?
O1 Mo1 Cs1 162.55(8) 7_565 5_656 ?
O3 Mo1 Cs1 117.294(11) 5_556 5_656 ?
O2 Mo1 Cs1 95.06(4) . 5_656 ?
Cs1 Mo1 Cs1 125.39(2) 5_666 5_656 ?
O7 Mo2 O6 104.73(13) . . ?
O7 Mo2 O2 96.89(14) . . ?
O6 Mo2 O2 99.67(14) . . ?
O7 Mo2 O3 99.69(14) . . ?
O6 Mo2 O3 92.08(14) . . ?
O2 Mo2 O3 156.52(16) . . ?
O7 Mo2 O1 91.49(12) . 5_556 ?
O6 Mo2 O1 159.77(11) . 5_556 ?
O2 Mo2 O1 90.11(12) . 5_556 ?
O3 Mo2 O1 73.02(12) . 5_556 ?
O7 Mo2 O1 161.78(11) . . ?
O6 Mo2 O1 92.48(11) . . ?
O2 Mo2 O1 73.94(12) . . ?
O3 Mo2 O1 85.38(12) . . ?
O1 Mo2 O1 73.14(11) 5_556 . ?
O7 Mo2 Cs1 146.72(10) . 5_656 ?
O6 Mo2 Cs1 48.60(9) . 5_656 ?
O2 Mo2 Cs1 106.23(11) . 5_656 ?
O3 Mo2 Cs1 67.01(11) . 5_656 ?
O1 Mo2 Cs1 111.70(7) 5_556 5_656 ?
O1 Mo2 Cs1 51.20(6) . 5_656 ?
O7 Mo2 Cs1 97.97(9) . . ?
O6 Mo2 Cs1 36.31(9) . . ?
O2 Mo2 Cs1 64.88(11) . . ?
O3 Mo2 Cs1 128.29(10) . . ?
O1 Mo2 Cs1 154.06(6) 5_556 . ?
O1 Mo2 Cs1 92.35(6) . . ?
Cs1 Mo2 Cs1 71.740(14) 5_656 . ?
Mo1 O1 Mo2 103.51(11) . 5_556 ?
Mo1 O1 Mo2 105.61(11) . . ?
Mo2 O1 Mo2 106.86(11) 5_556 . ?
Mo1 O1 Cs1 109.89(10) . 5_656 ?
Mo2 O1 Cs1 132.40(10) 5_556 5_656 ?
Mo2 O1 Cs1 95.85(8) . 5_656 ?
Mo2 O2 Mo2 152.6(2) 7_565 . ?
Mo2 O2 Mo1 103.64(11) 7_565 . ?
Mo2 O2 Mo1 103.64(11) . . ?
Mo2 O3 Mo2 150.4(2) . 7 ?
Mo2 O3 Mo1 102.87(10) . 5_556 ?
Mo2 O3 Mo1 102.87(10) 7 5_556 ?
Mo2 O3 Cs1 84.54(11) . 5_656 ?
Mo2 O3 Cs1 84.54(11) 7 5_656 ?
Mo1 O3 Cs1 141.29(15) 5_556 5_656 ?
Mo1 O4 Li1 159.2(4) . . ?
Mo1 O5 Li1 135.8(4) . 6_656 ?
Mo1 O5 Cs1 136.55(19) . . ?
Li1 O5 Cs1 87.7(3) 6_656 . ?
Mo1 O5 Cs1 92.91(6) . 5_656 ?
Li1 O5 Cs1 84.11(6) 6_656 5_656 ?
Cs1 O5 Cs1 91.63(6) . 5_656 ?
Mo1 O5 Cs1 92.91(6) . 5_666 ?
Li1 O5 Cs1 84.11(6) 6_656 5_666 ?
Cs1 O5 Cs1 91.63(6) . 5_666 ?
Cs1 O5 Cs1 167.64(12) 5_656 5_666 ?
Mo2 O6 Li1 128.7(3) . 2 ?
Mo2 O6 Cs1 107.76(12) . 5_656 ?
Li1 O6 Cs1 84.5(3) 2 5_656 ?
Mo2 O6 Cs1 125.40(12) . . ?
Li1 O6 Cs1 98.4(3) 2 . ?
Cs1 O6 Cs1 101.94(8) 5_656 . ?
Mo2 O7 Cs1 149.61(14) . 6_557 ?

_diffrn_measured_fraction_theta_max 0.999
_diffrn_reflns_theta_full        27.50
_diffrn_measured_fraction_theta_full 0.999
_refine_diff_density_max         0.775
_refine_diff_density_min         -0.732
_refine_diff_density_rms         0.188
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_1_CCDC2
_database_code_depnum_ccdc_archive 'CCDC 1823502'
_audit_update_record             
;
2018-02-11 deposited with the CCDC.
2018-05-10 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
; 
 ? 
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'Cs Mo3 Na O10'
_chemical_formula_weight         603.72

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           Orthorhombic
_symmetry_space_group_name_H-M   Pnma

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-x, y+1/2, -z'
'x+1/2, -y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, y, -z-1/2'
'x, -y-1/2, z'
'-x-1/2, y-1/2, z-1/2'

_cell_length_a                   7.750(5)
_cell_length_b                   7.612(5)
_cell_length_c                   15.600(10)
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_volume                     920.2(10)
_cell_formula_units_Z            4
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    1237
_cell_measurement_theta_min      2.61
_cell_measurement_theta_max      27.10

_exptl_crystal_description       block
_exptl_crystal_colour            colorless
_exptl_crystal_size_max          ?
_exptl_crystal_size_mid          ?
_exptl_crystal_size_min          ?
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    4.358
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1088
_exptl_absorpt_coefficient_mu    8.007
_exptl_absorpt_correction_type   none
_exptl_absorpt_correction_T_min  0.6153
_exptl_absorpt_correction_T_max  0.7456
_exptl_absorpt_process_details   ?

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            5253
_diffrn_reflns_av_R_equivalents  0.0434
_diffrn_reflns_av_sigmaI/netI    0.0348
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_theta_min         2.61
_diffrn_reflns_theta_max         27.57
_reflns_number_total             1134
_reflns_number_gt                949
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0157P)²+1.6313P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   ?
_refine_ls_hydrogen_treatment    ?
_refine_ls_extinction_method     SHELXL
_refine_ls_extinction_coef       0.00053(10)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_number_reflns         1134
_refine_ls_number_parameters     80
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0331
_refine_ls_R_factor_gt           0.0246
_refine_ls_wR_factor_ref         0.0480
_refine_ls_wR_factor_gt          0.0454
_refine_ls_goodness_of_fit_ref   1.030
_refine_ls_restrained_S_all      1.030
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Na1 Na 0.0574(4) 0.2500 0.27797(18) 0.0206(6) Uani 1 2 d S . .
Cs1 Cs 0.14463(6) 0.2500 0.64892(3) 0.02191(14) Uani 1 2 d S . .
Mo1 Mo -0.26711(7) 0.2500 0.44335(4) 0.01038(15) Uani 1 2 d S . .
Mo2 Mo 0.60951(5) -0.00122(5) 0.60060(3) 0.01008(12) Uani 1 1 d . . .
O1 O -0.3844(6) 0.2500 0.5743(3) 0.0123(10) Uani 1 2 d S . .
O2 O -0.3466(4) 0.0138(4) 0.4642(2) 0.0115(7) Uani 1 1 d . . .
O3 O 0.8189(4) -0.0329(4) 0.6299(2) 0.0191(8) Uani 1 1 d . . .
O4 O 0.5038(5) 0.0289(4) 0.6959(2) 0.0199(8) Uani 1 1 d . . .
O5 O 0.5572(6) -0.2500 0.5858(3) 0.0127(10) Uani 1 2 d S . .
O6 O -0.0689(6) 0.2500 0.4883(3) 0.0180(11) Uani 1 2 d S . .
O7 O -0.2292(6) 0.2500 0.3334(3) 0.0168(11) Uani 1 2 d S . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Na1 O7 2.384(5) . ?
Na1 O3 2.390(4) 3_656 ?
Na1 O3 2.390(4) 5_656 ?
Na1 O7 2.399(6) 6_656 ?
Na1 O4 2.524(4) 2_554 ?
Na1 O4 2.524(4) 8_665 ?
Na1 Mo2 3.594(3) 2_554 ?
Na1 Mo2 3.594(3) 8_665 ?
Na1 Mo1 3.603(3) . ?
Na1 Mo1 3.711(4) 6_656 ?
Na1 Mo2 3.720(3) 3_656 ?
Na1 Mo2 3.720(3) 5_656 ?
Cs1 O6 3.004(5) . ?
Cs1 O2 3.097(3) 5_556 ?
Cs1 O2 3.097(3) 3_556 ?
Cs1 O4 3.144(4) 4_456 ?
Cs1 O4 3.144(4) 6_557 ?
Cs1 O3 3.331(4) 1_455 ?
Cs1 O3 3.331(4) 7_465 ?
Cs1 O4 3.334(4) 7_565 ?
Cs1 O4 3.334(4) . ?
Cs1 Mo2 4.148(2) 7_565 ?
Cs1 Mo2 4.148(2) . ?
Cs1 Mo1 4.178(2) 5_556 ?
Mo1 O6 1.688(5) . ?
Mo1 O7 1.739(5) . ?
Mo1 O2 1.928(3) . ?
Mo1 O2 1.928(3) 7_565 ?
Mo1 O1 2.237(5) . ?
Mo1 O5 2.294(5) 5_556 ?
Mo1 Na1 3.711(4) 6_556 ?
Mo1 Cs1 4.178(2) 5_556 ?
Mo1 Cs1 4.178(2) 5_566 ?
Mo2 O3 1.703(3) . ?
Mo2 O4 1.712(4) . ?
Mo2 O5 1.9503(16) . ?
Mo2 O1 1.9562(15) 1_655 ?
Mo2 O2 2.158(3) 1_655 ?
Mo2 O2 2.276(3) 5_556 ?
Mo2 Na1 3.594(3) 2 ?
Mo2 Na1 3.720(3) 5_656 ?
Mo2 Cs1 4.359(2) 6_657 ?
O1 Mo2 1.9562(15) 7_465 ?
O1 Mo2 1.9562(15) 1_455 ?
O2 Mo2 2.158(3) 1_455 ?
O2 Mo2 2.276(3) 5_556 ?
O2 Cs1 3.097(3) 5_556 ?
O3 Na1 2.390(4) 5_656 ?
O3 Cs1 3.331(4) 1_655 ?
O4 Na1 2.524(4) 2 ?
O4 Cs1 3.144(4) 6_657 ?
O5 Mo2 1.9503(16) 7 ?
O5 Mo1 2.294(5) 5_556 ?
O7 Na1 2.399(6) 6_556 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O7 Na1 O3 98.94(15) . 3_656 ?
O7 Na1 O3 98.94(15) . 5_656 ?
O3 Na1 O3 87.5(2) 3_656 5_656 ?
O7 Na1 O7 154.86(18) . 6_656 ?
O3 Na1 O7 99.15(15) 3_656 6_656 ?
O3 Na1 O7 99.15(15) 5_656 6_656 ?
O7 Na1 O4 90.51(13) . 2_554 ?
O3 Na1 O4 164.10(16) 3_656 2_554 ?
O3 Na1 O4 78.40(12) 5_656 2_554 ?
O7 Na1 O4 76.24(12) 6_656 2_554 ?
O7 Na1 O4 90.51(13) . 8_665 ?
O3 Na1 O4 78.40(12) 3_656 8_665 ?
O3 Na1 O4 164.10(16) 5_656 8_665 ?
O7 Na1 O4 76.24(12) 6_656 8_665 ?
O4 Na1 O4 114.49(19) 2_554 8_665 ?
O7 Na1 Mo2 86.79(12) . 2_554 ?
O3 Na1 Mo2 166.26(12) 3_656 2_554 ?
O3 Na1 Mo2 104.05(10) 5_656 2_554 ?
O7 Na1 Mo2 71.96(12) 6_656 2_554 ?
O4 Na1 Mo2 25.65(8) 2_554 2_554 ?
O4 Na1 Mo2 89.13(12) 8_665 2_554 ?
O7 Na1 Mo2 86.79(12) . 8_665 ?
O3 Na1 Mo2 104.05(10) 3_656 8_665 ?
O3 Na1 Mo2 166.26(12) 5_656 8_665 ?
O7 Na1 Mo2 71.96(12) 6_656 8_665 ?
O4 Na1 Mo2 89.13(12) 2_554 8_665 ?
O4 Na1 Mo2 25.65(8) 8_665 8_665 ?
Mo2 Na1 Mo2 63.59(6) 2_554 8_665 ?
O7 Na1 Mo1 24.44(12) . . ?
O3 Na1 Mo1 81.35(12) 3_656 . ?
O3 Na1 Mo1 81.35(12) 5_656 . ?
O7 Na1 Mo1 179.30(16) 6_656 . ?
O4 Na1 Mo1 103.41(11) 2_554 . ?
O4 Na1 Mo1 103.41(11) 8_665 . ?
Mo2 Na1 Mo1 107.46(8) 2_554 . ?
Mo2 Na1 Mo1 107.46(8) 8_665 . ?
O7 Na1 Mo1 132.78(15) . 6_656 ?
O3 Na1 Mo1 114.35(12) 3_656 6_656 ?
O3 Na1 Mo1 114.35(12) 5_656 6_656 ?
O7 Na1 Mo1 22.08(11) 6_656 6_656 ?
O4 Na1 Mo1 66.23(10) 2_554 6_656 ?
O4 Na1 Mo1 66.23(10) 8_665 6_656 ?
Mo2 Na1 Mo1 54.24(5) 2_554 6_656 ?
Mo2 Na1 Mo1 54.24(5) 8_665 6_656 ?
Mo1 Na1 Mo1 157.22(9) . 6_656 ?
O7 Na1 Mo2 117.50(13) . 3_656 ?
O3 Na1 Mo2 20.56(9) 3_656 3_656 ?
O3 Na1 Mo2 76.56(11) 5_656 3_656 ?
O7 Na1 Mo2 83.72(12) 6_656 3_656 ?
O4 Na1 Mo2 144.79(12) 2_554 3_656 ?
O4 Na1 Mo2 87.75(9) 8_665 3_656 ?
Mo2 Na1 Mo2 155.52(9) 2_554 3_656 ?
Mo2 Na1 Mo2 111.94(5) 8_665 3_656 ?
Mo1 Na1 Mo2 96.88(8) . 3_656 ?
Mo1 Na1 Mo2 102.68(7) 6_656 3_656 ?
O7 Na1 Mo2 117.50(13) . 5_656 ?
O3 Na1 Mo2 76.56(11) 3_656 5_656 ?
O3 Na1 Mo2 20.56(9) 5_656 5_656 ?
O7 Na1 Mo2 83.72(12) 6_656 5_656 ?
O4 Na1 Mo2 87.75(9) 2_554 5_656 ?
O4 Na1 Mo2 144.79(12) 8_665 5_656 ?
Mo2 Na1 Mo2 111.94(5) 2_554 5_656 ?
Mo2 Na1 Mo2 155.52(9) 8_665 5_656 ?
Mo1 Na1 Mo2 96.88(8) . 5_656 ?
Mo1 Na1 Mo2 102.68(7) 6_656 5_656 ?
Mo2 Na1 Mo2 61.21(6) 3_656 5_656 ?
O6 Cs1 O2 78.64(10) . 5_556 ?
O6 Cs1 O2 78.64(10) . 3_556 ?
O2 Cs1 O2 80.81(12) 5_556 3_556 ?
O6 Cs1 O4 116.83(10) . 4_456 ?
O2 Cs1 O4 163.95(9) 5_556 4_456 ?
O2 Cs1 O4 105.49(9) 3_556 4_456 ?
O6 Cs1 O4 116.83(10) . 6_557 ?
O2 Cs1 O4 105.49(9) 5_556 6_557 ?
O2 Cs1 O4 163.95(9) 3_556 6_557 ?
O4 Cs1 O4 64.73(13) 4_456 6_557 ?
O6 Cs1 O3 60.55(9) . 1_455 ?
O2 Cs1 O3 85.02(9) 5_556 1_455 ?
O2 Cs1 O3 138.70(9) 3_556 1_455 ?
O4 Cs1 O3 98.72(10) 4_456 1_455 ?
O4 Cs1 O3 57.28(9) 6_557 1_455 ?
O6 Cs1 O3 60.55(9) . 7_465 ?
O2 Cs1 O3 138.70(9) 5_556 7_465 ?
O2 Cs1 O3 85.02(9) 3_556 7_465 ?
O4 Cs1 O3 57.28(9) 4_456 7_465 ?
O4 Cs1 O3 98.72(10) 6_557 7_465 ?
O3 Cs1 O3 80.55(13) 1_455 7_465 ?
O6 Cs1 O4 130.04(9) . 7_565 ?
O2 Cs1 O4 91.75(9) 5_556 7_565 ?
O2 Cs1 O4 51.40(9) 3_556 7_565 ?
O4 Cs1 O4 81.39(8) 4_456 7_565 ?
O4 Cs1 O4 113.00(7) 6_557 7_565 ?
O3 Cs1 O4 168.08(8) 1_455 7_565 ?
O3 Cs1 O4 109.02(9) 7_465 7_565 ?
O6 Cs1 O4 130.04(9) . . ?
O2 Cs1 O4 51.40(9) 5_556 . ?
O2 Cs1 O4 91.75(9) 3_556 . ?
O4 Cs1 O4 113.00(7) 4_456 . ?
O4 Cs1 O4 81.39(8) 6_557 . ?
O3 Cs1 O4 109.02(9) 1_455 . ?
O3 Cs1 O4 168.08(8) 7_465 . ?
O4 Cs1 O4 60.63(12) 7_565 . ?
O6 Cs1 Mo2 109.09(8) . 7_565 ?
O2 Cs1 Mo2 75.90(7) 5_556 7_565 ?
O2 Cs1 Mo2 32.73(6) 3_556 7_565 ?
O4 Cs1 Mo2 101.22(7) 4_456 7_565 ?
O4 Cs1 Mo2 133.48(7) 6_557 7_565 ?
O3 Cs1 Mo2 160.06(6) 1_455 7_565 ?
O3 Cs1 Mo2 110.12(7) 7_465 7_565 ?
O4 Cs1 Mo2 23.38(6) 7_565 7_565 ?
O4 Cs1 Mo2 63.10(7) . 7_565 ?
O6 Cs1 Mo2 109.09(8) . . ?
O2 Cs1 Mo2 32.73(6) 5_556 . ?
O2 Cs1 Mo2 75.90(7) 3_556 . ?
O4 Cs1 Mo2 133.48(7) 4_456 . ?
O4 Cs1 Mo2 101.22(7) 6_557 . ?
O3 Cs1 Mo2 110.12(7) 1_455 . ?
O3 Cs1 Mo2 160.06(6) 7_465 . ?
O4 Cs1 Mo2 63.10(7) 7_565 . ?
O4 Cs1 Mo2 23.38(6) . . ?
Mo2 Cs1 Mo2 54.91(4) 7_565 . ?
O6 Cs1 Mo1 80.66(4) . 5_556 ?
O2 Cs1 Mo1 25.65(6) 5_556 5_556 ?
O2 Cs1 Mo1 106.22(7) 3_556 5_556 ?
O4 Cs1 Mo1 146.27(6) 4_456 5_556 ?
O4 Cs1 Mo1 81.75(7) 6_557 5_556 ?
O3 Cs1 Mo1 63.43(7) 1_455 5_556 ?
O3 Cs1 Mo1 136.92(6) 7_465 5_556 ?
O4 Cs1 Mo1 110.23(7) 7_565 5_556 ?
O4 Cs1 Mo1 54.99(6) . 5_556 ?
Mo2 Cs1 Mo1 99.21(3) 7_565 5_556 ?
Mo2 Cs1 Mo1 47.167(14) . 5_556 ?
O6 Mo1 O7 104.8(2) . . ?
O6 Mo1 O2 102.75(11) . . ?
O7 Mo1 O2 102.72(10) . . ?
O6 Mo1 O2 102.75(11) . 7_565 ?
O7 Mo1 O2 102.72(10) . 7_565 ?
O2 Mo1 O2 137.65(18) . 7_565 ?
O6 Mo1 O1 89.5(2) . . ?
O7 Mo1 O1 165.7(2) . . ?
O2 Mo1 O1 73.51(10) . . ?
O2 Mo1 O1 73.51(10) 7_565 . ?
O6 Mo1 O5 166.9(2) . 5_556 ?
O7 Mo1 O5 88.3(2) . 5_556 ?
O2 Mo1 O5 73.76(10) . 5_556 ?
O2 Mo1 O5 73.76(10) 7_565 5_556 ?
O1 Mo1 O5 77.45(17) . 5_556 ?
O6 Mo1 Na1 70.25(18) . . ?
O7 Mo1 Na1 34.54(16) . . ?
O2 Mo1 Na1 110.10(9) . . ?
O2 Mo1 Na1 110.10(9) 7_565 . ?
O1 Mo1 Na1 159.72(13) . . ?
O5 Mo1 Na1 122.84(13) 5_556 . ?
O6 Mo1 Na1 136.01(17) . 6_556 ?
O7 Mo1 Na1 31.23(16) . 6_556 ?
O2 Mo1 Na1 92.28(10) . 6_556 ?
O2 Mo1 Na1 92.28(10) 7_565 6_556 ?
O1 Mo1 Na1 134.51(13) . 6_556 ?
O5 Mo1 Na1 57.07(12) 5_556 6_556 ?
Na1 Mo1 Na1 65.77(5) . 6_556 ?
O6 Mo1 Cs1 86.35(7) . 5_556 ?
O7 Mo1 Cs1 67.80(3) . 5_556 ?
O2 Mo1 Cs1 44.05(9) . 5_556 ?
O2 Mo1 Cs1 168.54(10) 7_565 5_556 ?
O1 Mo1 Cs1 114.02(2) . 5_556 ?
O5 Mo1 Cs1 98.88(5) 5_556 5_556 ?
Na1 Mo1 Cs1 66.095(19) . 5_556 ?
Na1 Mo1 Cs1 76.27(3) 6_556 5_556 ?
O6 Mo1 Cs1 86.35(7) . 5_566 ?
O7 Mo1 Cs1 67.80(3) . 5_566 ?
O2 Mo1 Cs1 168.54(10) . 5_566 ?
O2 Mo1 Cs1 44.05(10) 7_565 5_566 ?
O1 Mo1 Cs1 114.02(2) . 5_566 ?
O5 Mo1 Cs1 98.88(5) 5_556 5_566 ?
Na1 Mo1 Cs1 66.095(19) . 5_566 ?
Na1 Mo1 Cs1 76.27(3) 6_556 5_566 ?
Cs1 Mo1 Cs1 131.26(4) 5_556 5_566 ?
O3 Mo2 O4 103.96(17) . . ?
O3 Mo2 O5 95.30(17) . . ?
O4 Mo2 O5 97.66(18) . . ?
O3 Mo2 O1 99.90(18) . 1_655 ?
O4 Mo2 O1 93.57(17) . 1_655 ?
O5 Mo2 O1 158.33(19) . 1_655 ?
O3 Mo2 O2 97.02(15) . 1_655 ?
O4 Mo2 O2 157.55(15) . 1_655 ?
O5 Mo2 O2 88.13(16) . 1_655 ?
O1 Mo2 O2 74.82(15) 1_655 1_655 ?
O3 Mo2 O2 165.04(14) . 5_556 ?
O4 Mo2 O2 87.88(15) . 5_556 ?
O5 Mo2 O2 73.78(15) . 5_556 ?
O1 Mo2 O2 88.25(15) 1_655 5_556 ?
O2 Mo2 O2 72.87(13) 1_655 5_556 ?
O3 Mo2 Na1 93.52(13) . 2 ?
O4 Mo2 Na1 39.66(12) . 2 ?
O5 Mo2 Na1 60.31(14) . 2 ?
O1 Mo2 Na1 133.23(13) 1_655 2 ?
O2 Mo2 Na1 147.54(9) 1_655 2 ?
O2 Mo2 Na1 89.86(10) 5_556 2 ?
O3 Mo2 Na1 29.53(12) . 5_656 ?
O4 Mo2 Na1 87.59(13) . 5_656 ?
O5 Mo2 Na1 73.16(13) . 5_656 ?
O1 Mo2 Na1 125.99(14) 1_655 5_656 ?
O2 Mo2 Na1 114.81(10) 1_655 5_656 ?
O2 Mo2 Na1 145.67(8) 5_556 5_656 ?
Na1 Mo2 Na1 65.76(4) 2 5_656 ?
O3 Mo2 Cs1 147.57(12) . . ?
O4 Mo2 Cs1 50.59(12) . . ?
O5 Mo2 Cs1 106.77(13) . . ?
O1 Mo2 Cs1 66.93(13) 1_655 . ?
O2 Mo2 Cs1 106.96(8) 1_655 . ?
O2 Mo2 Cs1 47.36(8) 5_556 . ?
Na1 Mo2 Cs1 77.90(5) 2 . ?
Na1 Mo2 Cs1 138.15(5) 5_656 . ?
O3 Mo2 Cs1 76.22(12) . 6_657 ?
O4 Mo2 Cs1 36.20(12) . 6_657 ?
O5 Mo2 Cs1 123.03(14) . 6_657 ?
O1 Mo2 Cs1 75.96(13) 1_655 6_657 ?
O2 Mo2 Cs1 148.32(9) 1_655 6_657 ?
O2 Mo2 Cs1 118.18(8) 5_556 6_657 ?
Na1 Mo2 Cs1 64.12(5) 2 6_657 ?
Na1 Mo2 Cs1 73.95(5) 5_656 6_657 ?
Cs1 Mo2 Cs1 71.885(19) . 6_657 ?
Mo2 O1 Mo2 155.7(3) 7_465 1_455 ?
Mo2 O1 Mo1 101.60(12) 7_465 . ?
Mo2 O1 Mo1 101.60(12) 1_455 . ?
Mo1 O2 Mo2 105.42(14) . 1_455 ?
Mo1 O2 Mo2 104.48(13) . 5_556 ?
Mo2 O2 Mo2 107.13(13) 1_455 5_556 ?
Mo1 O2 Cs1 110.30(13) . 5_556 ?
Mo2 O2 Cs1 127.38(13) 1_455 5_556 ?
Mo2 O2 Cs1 99.91(11) 5_556 5_556 ?
Mo2 O3 Na1 129.91(19) . 5_656 ?
Mo2 O3 Cs1 130.86(16) . 1_655 ?
Na1 O3 Cs1 95.14(12) 5_656 1_655 ?
Mo2 O4 Na1 114.69(17) . 2 ?
Mo2 O4 Cs1 125.04(17) . 6_657 ?
Na1 O4 Cs1 97.17(13) 2 6_657 ?
Mo2 O4 Cs1 106.03(15) . . ?
Na1 O4 Cs1 112.26(14) 2 . ?
Cs1 O4 Cs1 100.88(10) 6_657 . ?
Mo2 O5 Mo2 152.3(3) . 7 ?
Mo2 O5 Mo1 103.14(13) . 5_556 ?
Mo2 O5 Mo1 103.14(13) 7 5_556 ?
Mo1 O6 Cs1 148.0(2) . . ?
Mo1 O7 Na1 121.0(2) . . ?
Mo1 O7 Na1 126.7(2) . 6_556 ?
Na1 O7 Na1 112.29(19) . 6_556 ?

_diffrn_measured_fraction_theta_max 0.992
_diffrn_reflns_theta_full        27.57
_diffrn_measured_fraction_theta_full 0.992
_refine_diff_density_max         0.855
_refine_diff_density_min         -1.593
_refine_diff_density_rms         0.204
